 
data_thebaite
 
_audit_creation_method            'SHELXL-2016/6'
_shelx_SHELXL_version_number      '2016/6'
_chemical_name_mineral            'thebaite' 
_chemical_compound_source         'Rowley mine, AZ'
_chemical_formula_sum
 'C2 Al0.90 Fe0.10 K1.04 N1.62 Na0.33 O12.76 P1.88' 
_chemical_formula_weight          387.56

loop_
 _atom_type_symbol
 _atom_type_description
 _atom_type_scat_dispersion_real
 _atom_type_scat_dispersion_imag
 _atom_type_scat_source
 'O'  'O'   0.0106   0.0060
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Al'  'Al'   0.0645   0.0514
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'P'  'P'   0.1023   0.0942
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'N'  'N'   0.0061   0.0033
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'C'  'C'   0.0033   0.0016
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'K'  'K'   0.2009   0.2494
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Fe'  'Fe'   0.3463   0.8444
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Na'  'Na'   0.0362   0.0249
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 
_space_group_crystal_system       monoclinic
_space_group_IT_number            14
_space_group_name_H-M_alt         'P 21/c'
_space_group_name_Hall            '-P 2ybc'
 
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
 
loop_
 _space_group_symop_operation_xyz
 'x, y, z'
 '-x, y+1/2, -z+1/2'
 '-x, -y, -z'
 'x, -y-1/2, z-1/2'
 
_cell_length_a                    11.156(9)
_cell_length_b                    6.234(6)
_cell_length_c                    18.651(16)
_cell_angle_alpha                 90
_cell_angle_beta                  102.927(15)
_cell_angle_gamma                 90
_cell_volume                      1264.2(19)
_cell_formula_units_Z             4
_cell_measurement_temperature     293(2)
_cell_measurement_reflns_used     1521
_cell_measurement_theta_min       2.24
_cell_measurement_theta_max       20.41
 
_exptl_crystal_description        'blade'
_exptl_crystal_colour             'colorless'
_exptl_crystal_density_diffrn     2.036          
_exptl_crystal_F_000              766
_exptl_crystal_size_max           0.070
_exptl_crystal_size_mid           0.013
_exptl_crystal_size_min           0.004
_exptl_absorpt_coefficient_mu     0.930
_shelx_estimated_absorpt_T_min    0.938
_shelx_estimated_absorpt_T_max    0.996
_diffrn_radiation_probe           'x-ray'
_diffrn_ambient_temperature       293(2)
_diffrn_radiation_wavelength      0.71073
_diffrn_radiation_type            MoK\a
_diffrn_measurement_device	  'three-circle diffractometer'
_diffrn_measurement_device_type   'Bruker D8 with CCD'
_diffrn_reflns_number             6266
_diffrn_reflns_av_unetI/netI      0.1165
_diffrn_reflns_av_R_equivalents   0.1725
_diffrn_reflns_limit_h_min        -12
_diffrn_reflns_limit_h_max        12
_diffrn_reflns_limit_k_min        -6
_diffrn_reflns_limit_k_max        6
_diffrn_reflns_limit_l_min        -20
_diffrn_reflns_limit_l_max        20
_diffrn_reflns_theta_min          3.227
_diffrn_reflns_theta_max          22.707
_diffrn_reflns_theta_full         22.707
_diffrn_measured_fraction_theta_max   0.991
_diffrn_measured_fraction_theta_full  0.991
_diffrn_reflns_Laue_measured_fraction_max    0.991
_diffrn_reflns_Laue_measured_fraction_full   0.991
_diffrn_reflns_point_group_measured_fraction_max   0.991
_diffrn_reflns_point_group_measured_fraction_full  0.991
_reflns_number_total              1679
_reflns_number_gt                 863
_reflns_threshold_expression      'I > 2σ(I)'
_reflns_Friedel_coverage          0.000
_reflns_Friedel_fraction_max      .
_reflns_Friedel_fraction_full     .
 
_reflns_special_details
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
 
_computing_structure_refinement 'SHELXL-2016/6 (Sheldrick, 2016)'
_refine_ls_structure_factor_coef  Fsqd
_refine_ls_matrix_type            full
_refine_ls_weighting_scheme       calc
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0810P)²] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_hydrogens    .
_refine_ls_hydrogen_treatment     undef
_refine_ls_extinction_method      none
_refine_ls_extinction_coef        .
_refine_ls_number_reflns          1679
_refine_ls_number_parameters      195
_refine_ls_number_restraints      0
_refine_ls_R_factor_all           0.1461
_refine_ls_R_factor_gt            0.0612
_refine_ls_wR_factor_ref          0.1720
_refine_ls_wR_factor_gt           0.1363
_refine_ls_goodness_of_fit_ref    1.017
_refine_ls_restrained_S_all       1.017
_refine_ls_shift/su_max           0.000
_refine_ls_shift/su_mean          0.000
 
loop_
 _atom_site_label
 _atom_site_type_symbol
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_U_iso_or_equiv
 _atom_site_adp_type
 _atom_site_occupancy
 _atom_site_site_symmetry_order  
 _atom_site_calc_flag
 _atom_site_refinement_flags_posn
 _atom_site_refinement_flags_adp
 _atom_site_refinement_flags_occupancy
 _atom_site_disorder_assembly
 _atom_site_disorder_group
K K 0.8845(2) 0.2489(6) 0.61514(14) 0.0521(13) Uani 0.67(2) 1 d . . P . .
Na Na 0.8845(2) 0.2489(6) 0.61514(14) 0.0521(13) Uani 0.33(2) 1 d . . P . .
N1 N 0.5148(5) 0.3750(11) 0.6664(3) 0.052(3) Uani 0.784(14) 1 d . . P . .
K1 K 0.5148(5) 0.3750(11) 0.6664(3) 0.052(3) Uani 0.216(14) 1 d . . P . .
N2 N 0.8162(7) 0.2278(13) 0.3420(4) 0.075(4) Uani 0.837(17) 1 d . . P . .
K2 K 0.8162(7) 0.2278(13) 0.3420(4) 0.075(4) Uani 0.163(17) 1 d . . P . .
P1 P 0.61541(18) 0.2443(5) 0.49820(12) 0.0234(7) Uani 1 1 d . . . . .
P2 P 0.3213(3) 0.1426(5) 0.30268(16) 0.0322(11) Uani 0.879(9) 1 d . . P . .
Al Al 0.31772(18) 0.2552(5) 0.46769(12) 0.0211(9) Uani 0.898(10) 1 d . . P . .
Fe Fe 0.31772(18) 0.2552(5) 0.46769(12) 0.0211(9) Uani 0.102(10) 1 d . . P . .
C1 C 0.1697(9) 0.2593(17) 0.5650(5) 0.031(2) Uani 1 1 d . . . . .
C2 C 0.0802(9) 0.2561(18) 0.4897(5) 0.031(2) Uani 1 1 d . . . . .
OH1 O 0.6093(5) 0.2382(11) 0.4128(3) 0.0339(16) Uani 1 1 d . . . . .
O2 O 0.6888(6) 0.4409(10) 0.5287(3) 0.0307(18) Uani 1 1 d . . . . .
O3 O 0.4852(4) 0.2516(11) 0.5100(3) 0.0257(14) Uani 1 1 d . . . . .
O4 O 0.6862(6) 0.0500(10) 0.5341(3) 0.0278(17) Uani 1 1 d . . . . .
OH5 O 0.3030(7) 0.3015(13) 0.2364(4) 0.065(3) Uani 1 1 d . . . . .
O6 O 0.4501(7) 0.0477(14) 0.3104(4) 0.045(2) Uani 0.879(9) 1 d . . P . .
O7 O 0.3208(5) 0.2761(11) 0.3688(3) 0.0351(18) Uani 1 1 d . . . . .
O8 O 0.2227(8) 0.9744(14) 0.2852(4) 0.049(3) Uani 0.879(9) 1 d . . P . .
O9 O 0.2813(5) 0.2537(11) 0.5648(3) 0.0309(15) Uani 1 1 d . . . . .
O10 O 0.1269(6) 0.2656(13) 0.6210(4) 0.050(2) Uani 1 1 d . . . . .
O11 O 0.1352(5) 0.2536(11) 0.4371(3) 0.0332(16) Uani 1 1 d . . . . .
O12 O 0.9678(5) 0.2520(13) 0.4832(3) 0.0433(18) Uani 1 1 d . . . . .
OWA O 0.986(3) 0.472(4) 0.756(2) 0.098(11) Uiso 0.61(10) 1 d . . P . .
OWB O 0.946(5) 0.507(6) 0.726(4) 0.089(17) Uiso 0.39(10) 1 d . . P . .
 
 
_geom_special_details
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
 
loop_
 _geom_bond_atom_site_label_1
 _geom_bond_atom_site_label_2
 _geom_bond_distance
 _geom_bond_site_symmetry_2
 _geom_bond_publ_flag
K OWB 2.59(5) . ?
K O10 2.684(7) 1_655 ?
K O4 2.687(7) . ?
K O2 2.687(7) . ?
K O8 2.796(8) 3_666 ?
K O12 2.819(7) . ?
K OWA 2.96(4) . ?
K OWA 3.05(3) 2_746 ?
K O11 3.243(8) 3_666 ?
K O11 3.274(8) 3_656 ?
K P1 3.292(4) . ?
K OWB 3.48(6) 2_746 ?
K1 O6 2.685(11) 3_656 ?
K1 O9 2.957(8) . ?
K1 O3 2.962(8) . ?
K1 O6 2.971(9) 4_566 ?
K1 OH1 3.000(9) 3_666 ?
K1 O7 3.011(9) 3_666 ?
K1 OH5 3.136(10) 3_666 ?
K1 OH5 3.143(10) 4_566 ?
K1 P2 3.500(8) 3_666 ?
K1 O2 3.573(9) . ?
K1 O8 3.599(11) 3_666 ?
K1 O6 3.636(11) 3_666 ?
K1 P1 3.653(6) . ?
K1 P2 3.686(7) 4_566 ?
K1 P2 3.690(8) 3_656 ?
K1 P1 3.895(7) 3_666 ?
K1 Fe 3.935(6) . ?
K1 O4 3.995(8) . ?
K1 O2 4.003(8) 3_666 ?
K2 O8 2.779(11) 2_645 ?
K2 O12 2.797(10) . ?
K2 OH1 2.905(9) . ?
K2 OWA 3.01(2) 4_565 ?
K2 OH5 3.178(11) 2_645 ?
K2 O10 3.185(12) 3_656 ?
K2 OWB 3.20(4) 4_565 ?
K2 O10 3.265(12) 3_666 ?
K2 C1 3.483(13) 3_656 ?
K2 C2 3.559(12) 1_655 ?
K2 OWB 3.60(3) 3_766 ?
K2 O11 3.607(9) 1_655 ?
K2 C1 3.624(13) 3_666 ?
K2 OWA 3.68(2) 3_766 ?
K2 P2 3.805(8) 2_655 ?
K2 OH5 3.979(11) 2_655 ?
K2 P1 4.054(8) . ?
K2 O6 4.136(11) 2_655 ?
K2 O6 4.149(11) . ?
K2 O2 4.256(10) . ?
P1 O2 1.513(7) . ?
P1 O4 1.517(7) . ?
P1 O3 1.518(5) . ?
P1 OH1 1.579(6) . ?
P1 O3 3.281(8) 3_656 ?
P1 O3 3.329(8) 3_666 ?
P1 O7 3.622(6) . ?
P1 O4 3.761(7) 3_656 ?
P1 O6 3.780(8) . ?
P2 O7 1.488(7) . ?
P2 O8 1.502(8) 1_545 ?
P2 O6 1.531(8) . ?
P2 OH5 1.561(8) . ?
P2 O4 3.291(7) 3_656 ?
P2 OH1 3.456(7) . ?
P2 OWB 3.64(6) 3_666 ?
P2 OWA 3.72(4) 4_465 ?
P2 O3 3.950(7) . ?
P2 O2 4.099(7) 3_666 ?
Fe O7 1.857(6) . ?
Fe O3 1.859(5) . ?
Fe O2 1.898(7) 3_666 ?
Fe O4 1.903(7) 3_656 ?
Fe O9 1.942(6) . ?
Fe O11 1.988(6) . ?
Fe OH1 3.623(6) . ?
Fe O3 3.748(7) 3_666 ?
Fe O8 3.763(8) 1_545 ?
Fe OH1 3.779(8) 3_656 ?
Fe O6 3.795(8) . ?
Fe O3 3.818(7) 3_656 ?
C1 O10 1.242(10) . ?
C1 O9 1.247(10) . ?
C1 C2 1.530(13) . ?
C1 O2 3.205(12) 3_666 ?
C1 OH5 3.233(11) 4_566 ?
C1 O4 3.324(12) 3_656 ?
C2 O12 1.233(10) 1_455 ?
C2 O11 1.268(10) . ?
C2 O2 3.274(12) 3_666 ?
C2 O4 3.339(12) 3_656 ?
OH1 O2 2.489(9) . ?
OH1 O3 2.516(8) . ?
OH1 O4 2.522(8) . ?
OH1 O6 2.588(10) . ?
OH1 O7 3.148(8) . ?
OH1 O9 3.293(10) 3_656 ?
OH1 O9 3.386(10) 3_666 ?
OH1 O3 3.631(10) 3_656 ?
OH1 O3 3.738(10) 3_666 ?
OH1 O4 4.066(9) 3_656 ?
OH1 OH5 4.164(10) 2_645 ?
O2 O4 2.439(8) . ?
O2 O3 2.514(8) . ?
O2 O7 2.622(9) 3_666 ?
O2 O9 2.652(9) 3_666 ?
O2 O11 2.707(9) 3_666 ?
O2 O3 2.709(8) 3_666 ?
O2 O12 3.602(9) . ?
O2 O4 3.799(9) 1_565 ?
O2 OWB 4.15(7) . ?
O3 O4 2.521(8) . ?
O3 O4 2.677(9) 3_656 ?
O3 O9 2.694(7) . ?
O3 O7 2.858(8) . ?
O3 O3 3.146(14) 3_666 ?
O3 O3 3.185(14) 3_656 ?
O3 O6 3.760(10) 3_656 ?
O4 O11 2.714(9) 3_656 ?
O4 O9 2.723(9) 3_656 ?
O4 O7 2.736(9) 3_656 ?
O4 O8 3.299(9) 3_666 ?
O4 O6 3.615(10) 3_656 ?
OH5 O7 2.437(9) . ?
OH5 O6 2.467(11) . ?
OH5 O8 2.481(11) 1_545 ?
OH5 O10 2.604(9) 4_565 ?
OH5 O9 3.175(10) 4_565 ?
OH5 OWB 3.23(4) 3_666 ?
OH5 O6 3.432(11) 2_655 ?
OH5 OWA 3.55(4) 3_666 ?
OH5 OWA 4.02(3) 4_465 ?
OH5 OWB 4.39(5) 4_465 ?
OH5 O8 4.426(13) . ?
O6 O7 2.449(10) . ?
O6 O8 2.516(11) 1_545 ?
O6 O6 4.141(10) 2_655 ?
O6 O6 4.141(10) 2_645 ?
O7 O8 2.530(10) 1_545 ?
O7 O11 2.667(8) . ?
O7 OWB 3.38(7) 3_666 ?
O7 OWA 4.00(5) 3_666 ?
O8 OWA 2.60(4) 4_475 ?
O8 OWB 3.04(6) 4_475 ?
O8 O10 3.418(10) 4_575 ?
O8 OWB 3.52(3) 3_666 ?
O8 OWA 3.60(2) 3_666 ?
O8 O11 3.640(11) 1_565 ?
O8 OWB 3.72(5) 3_676 ?
O8 OWA 4.14(4) 3_676 ?
O10 OWA 3.39(2) 2_646 ?
O10 OWB 3.46(3) 1_455 ?
O10 OWA 3.49(2) 1_455 ?
O10 OWB 3.52(4) 2_646 ?
O11 OWB 3.33(7) 3_666 ?
OWA OWB 0.66(4) . ?
OWA OWB 3.00(5) 2_746 ?
OWA OWA 3.145(6) 2_746 ?
OWA OWA 3.145(6) 2_756 ?
OWA OWB 3.42(5) 2_756 ?
OWB OWB 3.39(6) 2_746 ?
OWB OWB 3.39(6) 2_756 ?
 
loop_
 _geom_angle_atom_site_label_1
 _geom_angle_atom_site_label_2
 _geom_angle_atom_site_label_3
 _geom_angle
 _geom_angle_site_symmetry_1
 _geom_angle_site_symmetry_3
 _geom_angle_publ_flag
OWB K O10 82.0(10) . 1_655 ?
OWB K O4 140.6(10) . . ?
O10 K O4 137.4(2) 1_655 . ?
OWB K O2 103.7(15) . . ?
O10 K O2 133.1(2) 1_655 . ?
O4 K O2 53.99(18) . . ?
OWB K O8 81.4(9) . 3_666 ?
O10 K O8 124.7(2) 1_655 3_666 ?
O4 K O8 74.0(2) . 3_666 ?
O2 K O8 102.1(2) . 3_666 ?
OWB K O12 128.0(8) . . ?
O10 K O12 60.59(19) 1_655 . ?
O4 K O12 84.4(2) . . ?
O2 K O12 81.7(2) . . ?
O8 K O12 149.0(3) 3_666 . ?
OWB K OWA 11.4(11) . . ?
O10 K OWA 76.4(6) 1_655 . ?
O4 K OWA 144.9(5) . . ?
O2 K OWA 114.8(8) . . ?
O8 K OWA 77.3(5) 3_666 . ?
O12 K OWA 129.4(4) . . ?
OWB K OWA 74.1(11) . 2_746 ?
O10 K OWA 72.2(6) 1_655 2_746 ?
O4 K OWA 111.6(8) . 2_746 ?
O2 K OWA 154.6(5) . 2_746 ?
O8 K OWA 52.5(6) 3_666 2_746 ?
O12 K OWA 120.1(4) . 2_746 ?
OWA K OWA 63.06(13) . 2_746 ?
OWB K O11 68.7(14) . 3_666 ?
O10 K O11 88.6(2) 1_655 3_666 ?
O4 K O11 106.28(19) . 3_666 ?
O2 K O11 53.31(18) . 3_666 ?
O8 K O11 131.7(2) 3_666 3_666 ?
O12 K O11 75.2(2) . 3_666 ?
OWA K O11 78.7(8) . 3_666 ?
OWA K O11 140.0(9) 2_746 3_666 ?
OWB K O11 145.0(15) . 3_656 ?
O10 K O11 92.8(2) 1_655 3_656 ?
O4 K O11 53.06(17) . 3_656 ?
O2 K O11 104.85(19) . 3_656 ?
O8 K O11 73.2(2) 3_666 3_656 ?
O12 K O11 76.1(2) . 3_656 ?
OWA K O11 134.5(8) . 3_656 ?
OWA K O11 71.5(8) 2_746 3_656 ?
O11 K O11 146.1(2) 3_666 3_656 ?
OWB K P1 125.0(14) . . ?
O10 K P1 142.03(18) 1_655 . ?
O4 K P1 27.06(14) . . ?
O2 K P1 26.95(15) . . ?
O8 K P1 88.51(18) 3_666 . ?
O12 K P1 81.47(15) . . ?
OWA K P1 134.6(7) . . ?
OWA K P1 136.0(8) 2_746 . ?
O11 K P1 79.56(13) 3_666 . ?
O11 K P1 78.70(13) 3_656 . ?
OWB K OWB 66.0(7) . 2_746 ?
O10 K OWB 68.3(6) 1_655 2_746 ?
O4 K OWB 120.1(10) . 2_746 ?
O2 K OWB 156.7(5) . 2_746 ?
O8 K OWB 56.8(7) 3_666 2_746 ?
O12 K OWB 121.4(5) . 2_746 ?
OWA K OWB 54.8(7) . 2_746 ?
OWA K OWB 8.9(7) 2_746 2_746 ?
O11 K OWB 131.1(10) 3_666 2_746 ?
O11 K OWB 79.9(10) 3_656 2_746 ?
P1 K OWB 143.3(8) . 2_746 ?
O6 K1 O9 85.9(3) 3_656 . ?
O6 K1 O3 83.3(3) 3_656 . ?
O9 K1 O3 54.15(18) . . ?
O6 K1 O6 94.0(3) 3_656 4_566 ?
O9 K1 O6 105.3(3) . 4_566 ?
O3 K1 O6 159.3(3) . 4_566 ?
O6 K1 OH1 154.6(3) 3_656 3_666 ?
O9 K1 OH1 69.3(2) . 3_666 ?
O3 K1 OH1 77.7(2) . 3_666 ?
O6 K1 OH1 97.8(3) 4_566 3_666 ?
O6 K1 O7 132.1(3) 3_656 3_666 ?
O9 K1 O7 122.5(3) . 3_666 ?
O3 K1 O7 85.0(2) . 3_666 ?
O6 K1 O7 111.3(3) 4_566 3_666 ?
OH1 K1 O7 63.2(2) 3_666 3_666 ?
O6 K1 OH5 119.0(3) 3_656 3_666 ?
O9 K1 OH5 154.0(3) . 3_666 ?
O3 K1 OH5 130.6(3) . 3_666 ?
O6 K1 OH5 68.3(2) 4_566 3_666 ?
OH1 K1 OH5 86.3(3) 3_666 3_666 ?
O7 K1 OH5 46.7(2) 3_666 3_666 ?
O6 K1 OH5 71.7(3) 3_656 4_566 ?
O9 K1 OH5 62.7(2) . 4_566 ?
O3 K1 OH5 112.9(3) . 4_566 ?
O6 K1 OH5 47.5(2) 4_566 4_566 ?
OH1 K1 OH5 100.3(2) 3_666 4_566 ?
O7 K1 OH5 153.5(3) 3_666 4_566 ?
OH5 K1 OH5 115.8(2) 3_666 4_566 ?
O6 K1 P2 139.9(3) 3_656 3_666 ?
O9 K1 P2 132.7(2) . 3_666 ?
O3 K1 P2 108.9(2) . 3_666 ?
O6 K1 P2 86.3(2) 4_566 3_666 ?
OH1 K1 P2 63.71(19) 3_666 3_666 ?
O7 K1 P2 25.01(14) 3_666 3_666 ?
OH5 K1 P2 26.49(15) 3_666 3_666 ?
OH5 K1 P2 130.2(2) 4_566 3_666 ?
O6 K1 O2 98.4(2) 3_656 . ?
O9 K1 O2 96.4(2) . . ?
O3 K1 O2 44.02(16) . . ?
O6 K1 O2 155.8(3) 4_566 . ?
OH1 K1 O2 79.5(2) 3_666 . ?
O7 K1 O2 45.95(18) 3_666 . ?
OH5 K1 O2 87.4(2) 3_666 . ?
OH5 K1 O2 156.8(3) 4_566 . ?
P2 K1 O2 70.84(16) 3_666 . ?
O6 K1 O8 44.3(2) 3_656 3_666 ?
O9 K1 O8 123.8(3) . 3_666 ?
O3 K1 O8 89.7(2) . 3_666 ?
O6 K1 O8 102.7(3) 4_566 3_666 ?
OH1 K1 O8 150.4(3) 3_666 3_666 ?
O7 K1 O8 89.5(2) 3_666 3_666 ?
OH5 K1 O8 81.9(2) 3_666 3_666 ?
OH5 K1 O8 109.2(3) 4_566 3_666 ?
P2 K1 O8 96.5(2) 3_666 3_666 ?
O2 K1 O8 73.0(2) . 3_666 ?
O6 K1 O6 160.8(3) 3_656 3_666 ?
O9 K1 O6 112.7(3) . 3_666 ?
O3 K1 O6 111.1(2) . 3_666 ?
O6 K1 O6 76.9(2) 4_566 3_666 ?
OH1 K1 O6 44.6(2) 3_666 3_666 ?
O7 K1 O6 41.94(19) 3_666 3_666 ?
OH5 K1 O6 41.9(2) 3_666 3_666 ?
OH5 K1 O6 111.6(2) 4_566 3_666 ?
P2 K1 O6 24.68(14) 3_666 3_666 ?
O2 K1 O6 84.9(2) . 3_666 ?
O8 K1 O6 120.6(2) 3_666 3_666 ?
O6 K1 P1 81.8(2) 3_656 . ?
O9 K1 P1 77.77(18) . . ?
O3 K1 P1 23.71(11) . . ?
O6 K1 P1 174.7(3) 4_566 . ?
OH1 K1 P1 87.29(18) 3_666 . ?
O7 K1 P1 69.80(17) 3_666 . ?
OH5 K1 P1 110.8(2) 3_666 . ?
OH5 K1 P1 133.1(2) 4_566 . ?
P2 K1 P1 94.79(15) 3_666 . ?
O2 K1 P1 24.13(12) . . ?
O8 K1 P1 72.01(17) 3_666 . ?
O6 K1 P1 106.11(19) 3_666 . ?
O6 K1 P2 86.9(2) 3_656 4_566 ?
O9 K1 P2 82.34(18) . 4_566 ?
O3 K1 P2 135.9(2) . 4_566 ?
O6 K1 P2 23.60(17) 4_566 4_566 ?
OH1 K1 P2 94.98(19) 3_666 4_566 ?
O7 K1 P2 130.6(2) 3_666 4_566 ?
OH5 K1 P2 91.4(2) 3_666 4_566 ?
OH5 K1 P2 24.83(15) 4_566 4_566 ?
P2 K1 P2 106.08(17) 3_666 4_566 ?
O2 K1 P2 174.5(2) . 4_566 ?
O8 K1 P2 112.2(2) 3_666 4_566 ?
O6 K1 P2 90.66(18) 3_666 4_566 ?
P1 K1 P2 157.74(19) . 4_566 ?
O6 K1 P2 21.13(18) 3_656 3_656 ?
O9 K1 P2 102.2(2) . 3_656 ?
O3 K1 P2 82.5(2) . 3_656 ?
O6 K1 P2 102.3(2) 4_566 3_656 ?
OH1 K1 P2 159.7(2) 3_666 3_656 ?
O7 K1 P2 111.2(2) 3_666 3_656 ?
OH5 K1 P2 103.7(2) 3_666 3_656 ?
OH5 K1 P2 91.2(2) 4_566 3_656 ?
P2 K1 P2 120.22(19) 3_666 3_656 ?
O2 K1 P2 83.27(17) . 3_656 ?
O8 K1 P2 23.74(14) 3_666 3_656 ?
O6 K1 P2 144.2(2) 3_666 3_656 ?
P1 K1 P2 72.69(13) . 3_656 ?
P2 K1 P2 102.26(17) 4_566 3_656 ?
O6 K1 P1 137.8(3) 3_656 3_666 ?
O9 K1 P1 62.01(17) . 3_666 ?
O3 K1 P1 56.12(17) . 3_666 ?
O6 K1 P1 119.4(2) 4_566 3_666 ?
OH1 K1 P1 21.93(13) 3_666 3_666 ?
O7 K1 P1 61.71(16) 3_666 3_666 ?
OH5 K1 P1 98.2(2) 3_666 3_666 ?
OH5 K1 P1 111.0(2) 4_566 3_666 ?
P2 K1 P1 72.26(14) 3_666 3_666 ?
O2 K1 P1 61.98(15) . 3_666 ?
O8 K1 P1 134.9(2) 3_666 3_666 ?
O6 K1 P1 60.14(16) 3_666 3_666 ?
P1 K1 P1 65.86(12) . 3_666 ?
P2 K1 P1 112.89(17) 4_566 3_666 ?
P2 K1 P1 137.76(17) 3_656 3_666 ?
O6 K1 Fe 89.8(2) 3_656 . ?
O9 K1 Fe 28.48(12) . . ?
O3 K1 Fe 26.84(11) . . ?
O6 K1 Fe 133.2(2) 4_566 . ?
OH1 K1 Fe 65.77(17) 3_666 . ?
O7 K1 Fe 99.86(19) 3_666 . ?
OH5 K1 Fe 145.1(2) 3_666 . ?
OH5 K1 Fe 90.7(2) 4_566 . ?
P2 K1 Fe 118.66(17) 3_666 . ?
O2 K1 Fe 67.90(15) . . ?
O8 K1 Fe 111.9(2) 3_666 . ?
O6 K1 Fe 108.83(19) 3_666 . ?
P1 K1 Fe 50.43(10) . . ?
P2 K1 Fe 110.72(16) 4_566 . ?
P2 K1 Fe 97.71(16) 3_656 . ?
P1 K1 Fe 48.85(10) 3_666 . ?
O6 K1 O4 61.9(2) 3_656 . ?
O9 K1 O4 87.1(2) . . ?
O3 K1 O4 39.06(15) . . ?
O6 K1 O4 152.5(3) 4_566 . ?
OH1 K1 O4 109.6(2) 3_666 . ?
O7 K1 O4 80.4(2) 3_666 . ?
OH5 K1 O4 110.2(2) 3_666 . ?
OH5 K1 O4 126.0(3) 4_566 . ?
P2 K1 O4 103.47(18) 3_666 . ?
O2 K1 O4 37.08(14) . . ?
O8 K1 O4 51.17(16) 3_666 . ?
O6 K1 O4 121.5(2) 3_666 . ?
P1 K1 O4 22.31(10) . . ?
P2 K1 O4 147.8(2) 4_566 . ?
P2 K1 O4 50.52(13) 3_656 . ?
P1 K1 O4 88.15(16) 3_666 . ?
Fe K1 O4 64.26(14) . . ?
O6 K1 O2 117.4(3) 3_656 3_666 ?
O9 K1 O2 41.49(17) . 3_666 ?
O3 K1 O2 42.60(16) . 3_666 ?
O6 K1 O2 124.9(3) 4_566 3_666 ?
OH1 K1 O2 38.38(17) 3_666 3_666 ?
O7 K1 O2 81.0(2) 3_666 3_666 ?
OH5 K1 O2 120.2(3) 3_666 3_666 ?
OH5 K1 O2 98.7(2) 4_566 3_666 ?
P2 K1 O2 94.17(18) 3_666 3_666 ?
O2 K1 O2 66.59(19) . 3_666 ?
O8 K1 O2 131.8(2) 3_666 3_666 ?
O6 K1 O2 81.29(19) 3_666 3_666 ?
P1 K1 O2 60.27(14) . 3_666 ?
P2 K1 O2 109.55(18) 4_566 3_666 ?
P2 K1 O2 123.60(18) 3_656 3_666 ?
P1 K1 O2 22.03(11) 3_666 3_666 ?
Fe K1 O2 27.65(11) . 3_666 ?
O4 K1 O2 80.60(17) . 3_666 ?
O8 K2 O12 136.0(4) 2_645 . ?
O8 K2 OH1 112.8(3) 2_645 . ?
O12 K2 OH1 86.9(3) . . ?
O8 K2 OWA 76.6(6) 2_645 4_565 ?
O12 K2 OWA 101.9(9) . 4_565 ?
OH1 K2 OWA 155.4(8) . 4_565 ?
O8 K2 OH5 95.7(3) 2_645 2_645 ?
O12 K2 OH5 125.5(3) . 2_645 ?
OH1 K2 OH5 86.3(3) . 2_645 ?
OWA K2 OH5 69.9(9) 4_565 2_645 ?
O8 K2 O10 134.8(3) 2_645 3_656 ?
O12 K2 O10 78.4(3) . 3_656 ?
OH1 K2 O10 93.6(3) . 3_656 ?
OWA K2 O10 66.3(4) 4_565 3_656 ?
OH5 K2 O10 48.3(2) 2_645 3_656 ?
O8 K2 OWB 71.6(8) 2_645 4_565 ?
O12 K2 OWB 112.9(13) . 4_565 ?
OH1 K2 OWB 147.1(11) . 4_565 ?
OWA K2 OWB 11.7(7) 4_565 4_565 ?
OH5 K2 OWB 60.9(11) 2_645 4_565 ?
O10 K2 OWB 66.9(6) 3_656 4_565 ?
O8 K2 O10 68.3(3) 2_645 3_666 ?
O12 K2 O10 72.6(3) . 3_666 ?
OH1 K2 O10 91.1(3) . 3_666 ?
OWA K2 O10 113.4(7) 4_565 3_666 ?
OH5 K2 O10 161.4(3) 2_645 3_666 ?
O10 K2 O10 150.3(3) 3_656 3_666 ?
OWB K2 O10 119.2(8) 4_565 3_666 ?
O8 K2 C1 152.7(4) 2_645 3_656 ?
O12 K2 C1 68.2(3) . 3_656 ?
OH1 K2 C1 75.2(3) . 3_656 ?
OWA K2 C1 86.7(5) 4_565 3_656 ?
OH5 K2 C1 57.9(2) 2_645 3_656 ?
O10 K2 C1 20.86(18) 3_656 3_656 ?
OWB K2 C1 87.7(6) 4_565 3_656 ?
O10 K2 C1 138.9(3) 3_666 3_656 ?
O8 K2 C2 125.3(4) 2_645 1_655 ?
O12 K2 C2 17.67(19) . 1_655 ?
OH1 K2 C2 104.6(3) . 1_655 ?
OWA K2 C2 85.7(10) 4_565 1_655 ?
OH5 K2 C2 125.9(3) 2_645 1_655 ?
O10 K2 C2 77.9(3) 3_656 1_655 ?
OWB K2 C2 97.1(13) 4_565 1_655 ?
O10 K2 C2 72.6(3) 3_666 1_655 ?
C1 K2 C2 73.8(3) 3_656 1_655 ?
O8 K2 OWB 55.2(13) 2_645 3_766 ?
O12 K2 OWB 88.3(12) . 3_766 ?
OH1 K2 OWB 151.1(7) . 3_766 ?
OWA K2 OWB 53.1(8) 4_565 3_766 ?
OH5 K2 OWB 119.2(7) 2_645 3_766 ?
O10 K2 OWB 113.2(9) 3_656 3_766 ?
OWB K2 OWB 59.4(9) 4_565 3_766 ?
O10 K2 OWB 60.4(5) 3_666 3_766 ?
C1 K2 OWB 128.5(11) 3_656 3_766 ?
C2 K2 OWB 72.7(12) 1_655 3_766 ?
O8 K2 O11 110.1(3) 2_645 1_655 ?
O12 K2 O11 38.04(18) . 1_655 ?
OH1 K2 O11 124.9(3) . 1_655 ?
OWA K2 O11 67.2(10) 4_565 1_655 ?
OH5 K2 O11 121.9(3) 2_645 1_655 ?
O10 K2 O11 79.0(2) 3_656 1_655 ?
OWB K2 O11 78.9(13) 4_565 1_655 ?
O10 K2 O11 74.3(2) 3_666 1_655 ?
C1 K2 O11 82.2(2) 3_656 1_655 ?
C2 K2 O11 20.37(16) 1_655 1_655 ?
OWB K2 O11 55.1(12) 3_766 1_655 ?
O8 K2 C1 84.4(3) 2_645 3_666 ?
O12 K2 C1 63.2(3) . 3_666 ?
OH1 K2 C1 73.5(3) . 3_666 ?
OWA K2 C1 130.9(8) 4_565 3_666 ?
OH5 K2 C1 158.0(3) 2_645 3_666 ?
O10 K2 C1 139.8(3) 3_656 3_666 ?
OWB K2 C1 138.3(9) 4_565 3_666 ?
O10 K2 C1 19.91(18) 3_666 3_666 ?
C1 K2 C1 122.6(3) 3_656 3_666 ?
C2 K2 C1 69.3(3) 1_655 3_666 ?
OWB K2 C1 78.9(5) 3_766 3_666 ?
O11 K2 C1 78.0(2) 1_655 3_666 ?
O8 K2 OWA 44.8(8) 2_645 3_766 ?
O12 K2 OWA 97.8(8) . 3_766 ?
OH1 K2 OWA 147.2(6) . 3_766 ?
OWA K2 OWA 55.02(17) 4_565 3_766 ?
OH5 K2 OWA 115.7(5) 2_645 3_766 ?
O10 K2 OWA 119.1(6) 3_656 3_766 ?
OWB K2 OWA 59.1(9) 4_565 3_766 ?
O10 K2 OWA 60.1(4) 3_666 3_766 ?
C1 K2 OWA 136.5(7) 3_656 3_766 ?
C2 K2 OWA 82.7(8) 1_655 3_766 ?
OWB K2 OWA 10.4(7) 3_766 3_766 ?
O11 K2 OWA 65.5(8) 1_655 3_766 ?
C1 K2 OWA 79.7(4) 3_666 3_766 ?
O8 K2 P2 19.43(17) 2_645 2_655 ?
O12 K2 P2 133.9(3) . 2_655 ?
OH1 K2 P2 94.1(2) . 2_655 ?
OWA K2 P2 95.9(6) 4_565 2_655 ?
OH5 K2 P2 100.4(2) 2_645 2_655 ?
O10 K2 P2 147.1(3) 3_656 2_655 ?
OWB K2 P2 90.2(8) 4_565 2_655 ?
O10 K2 P2 61.36(19) 3_666 2_655 ?
C1 K2 P2 155.8(3) 3_656 2_655 ?
C2 K2 P2 130.4(3) 1_655 2_655 ?
OWB K2 P2 69.4(12) 3_766 2_655 ?
O11 K2 P2 121.0(2) 1_655 2_655 ?
C1 K2 P2 73.0(2) 3_666 2_655 ?
OWA K2 P2 59.6(8) 3_766 2_655 ?
O8 K2 OH5 38.1(2) 2_645 2_655 ?
O12 K2 OH5 112.3(3) . 2_655 ?
OH1 K2 OH5 85.0(3) . 2_655 ?
OWA K2 OH5 111.9(5) 4_565 2_655 ?
OH5 K2 OH5 120.7(3) 2_645 2_655 ?
O10 K2 OH5 169.1(3) 3_656 2_655 ?
OWB K2 OH5 109.0(7) 4_565 2_655 ?
O10 K2 OH5 40.65(18) 3_666 2_655 ?
C1 K2 OH5 160.2(3) 3_656 2_655 ?
C2 K2 OH5 113.0(3) 1_655 2_655 ?
OWB K2 OH5 70.6(10) 3_766 2_655 ?
O11 K2 OH5 110.6(3) 1_655 2_655 ?
C1 K2 OH5 50.1(2) 3_666 2_655 ?
OWA K2 OH5 63.2(6) 3_766 2_655 ?
P2 K2 OH5 23.00(12) 2_655 2_655 ?
O8 K2 P1 126.4(3) 2_645 . ?
O12 K2 P1 68.7(2) . . ?
OH1 K2 P1 18.17(12) . . ?
OWA K2 P1 155.3(5) 4_565 . ?
OH5 K2 P1 96.3(2) 2_645 . ?
O10 K2 P1 89.1(2) 3_656 . ?
OWB K2 P1 154.2(7) 4_565 . ?
O10 K2 P1 86.3(2) 3_666 . ?
C1 K2 P1 68.6(2) 3_656 . ?
C2 K2 P1 86.4(2) 1_655 . ?
OWB K2 P1 144.5(7) 3_766 . ?
O11 K2 P1 106.8(2) 1_655 . ?
C1 K2 P1 66.8(2) 3_666 . ?
OWA K2 P1 146.5(4) 3_766 . ?
P2 K2 P1 107.01(19) 2_655 . ?
OH5 K2 P1 92.8(2) 2_655 . ?
O8 K2 O6 36.4(2) 2_645 2_655 ?
O12 K2 O6 144.2(3) . 2_655 ?
OH1 K2 O6 77.3(2) . 2_655 ?
OWA K2 O6 105.8(8) 4_565 2_655 ?
OH5 K2 O6 85.7(2) 2_645 2_655 ?
O10 K2 O6 133.8(3) 3_656 2_655 ?
OWB K2 O6 96.9(11) 4_565 2_655 ?
O10 K2 O6 75.8(2) 3_666 2_655 ?
C1 K2 O6 135.1(3) 3_656 2_655 ?
C2 K2 O6 148.3(3) 1_655 2_655 ?
OWB K2 O6 90.5(12) 3_766 2_655 ?
O11 K2 O6 142.6(3) 1_655 2_655 ?
C1 K2 O6 81.4(2) 3_666 2_655 ?
OWA K2 O6 80.4(8) 3_766 2_655 ?
P2 K2 O6 21.72(12) 2_655 2_655 ?
OH5 K2 O6 35.33(17) 2_655 2_655 ?
P1 K2 O6 93.10(19) . 2_655 ?
O8 K2 O6 93.9(3) 2_645 . ?
O12 K2 O6 121.2(3) . . ?
OH1 K2 O6 38.16(18) . . ?
OWA K2 O6 121.9(9) 4_565 . ?
OH5 K2 O6 53.9(2) 2_645 . ?
O10 K2 O6 84.9(2) 3_656 . ?
OWB K2 O6 111.0(12) 4_565 . ?
O10 K2 O6 115.5(3) 3_666 . ?
C1 K2 O6 76.6(2) 3_656 . ?
C2 K2 O6 137.9(3) 1_655 . ?
OWB K2 O6 148.8(13) 3_766 . ?
O11 K2 O6 156.0(3) 1_655 . ?
C1 K2 O6 104.1(3) 3_666 . ?
OWA K2 O6 138.5(8) 3_766 . ?
P2 K2 O6 81.67(19) 2_655 . ?
OH5 K2 O6 87.3(2) 2_655 . ?
P1 K2 O6 54.87(14) . . ?
O6 K2 O6 59.98(16) 2_655 . ?
O8 K2 O2 120.6(3) 2_645 . ?
O12 K2 O2 57.0(2) . . ?
OH1 K2 O2 34.58(17) . . ?
OWA K2 O2 158.5(9) 4_565 . ?
OH5 K2 O2 117.1(3) 2_645 . ?
O10 K2 O2 102.2(2) 3_656 . ?
OWB K2 O2 167.5(9) 4_565 . ?
O10 K2 O2 67.0(2) 3_666 . ?
C1 K2 O2 81.4(2) 3_656 . ?
C2 K2 O2 73.8(2) 1_655 . ?
OWB K2 O2 123.7(7) 3_766 . ?
O11 K2 O2 93.3(2) 1_655 . ?
C1 K2 O2 47.2(2) 3_666 . ?
OWA K2 O2 126.5(4) 3_766 . ?
P2 K2 O2 102.3(2) 2_655 . ?
OH5 K2 O2 82.8(2) 2_655 . ?
P1 K2 O2 20.79(10) . . ?
O6 K2 O2 95.3(2) 2_655 . ?
O6 K2 O2 72.71(18) . . ?
O2 P1 O4 107.2(3) . . ?
O2 P1 O3 112.1(4) . . ?
O4 P1 O3 112.3(4) . . ?
O2 P1 OH1 107.2(4) . . ?
O4 P1 OH1 109.1(4) . . ?
O3 P1 OH1 108.7(3) . . ?
O2 P1 O3 158.7(3) . 3_656 ?
O4 P1 O3 53.6(3) . 3_656 ?
O3 P1 O3 72.9(3) . 3_656 ?
OH1 P1 O3 89.6(3) . 3_656 ?
O2 P1 K 53.6(3) . . ?
O4 P1 K 53.7(3) . . ?
O3 P1 K 131.6(2) . . ?
OH1 P1 K 119.7(2) . . ?
O3 P1 K 106.91(14) 3_656 . ?
O2 P1 O3 53.2(3) . 3_666 ?
O4 P1 O3 155.6(3) . 3_666 ?
O3 P1 O3 69.8(3) . 3_666 ?
OH1 P1 O3 92.2(3) . 3_666 ?
O3 P1 O3 141.17(17) 3_656 3_666 ?
K P1 O3 105.69(14) . 3_666 ?
O2 P1 O7 122.7(3) . . ?
O4 P1 O7 130.0(3) . . ?
O3 P1 O7 48.7(2) . . ?
OH1 P1 O7 60.1(2) . . ?
O3 P1 O7 76.72(15) 3_656 . ?
K P1 O7 176.35(16) . . ?
O3 P1 O7 70.80(15) 3_666 . ?
O2 P1 K1 75.0(3) . . ?
O4 P1 K1 91.6(3) . . ?
O3 P1 K1 51.7(2) . . ?
OH1 P1 K1 156.8(3) . . ?
O3 P1 K1 94.75(15) 3_656 . ?
K P1 K1 80.73(12) . . ?
O3 P1 K1 70.36(14) 3_666 . ?
O7 P1 K1 98.79(15) . . ?
O2 P1 O4 147.7(3) . 3_656 ?
O4 P1 O4 92.3(3) . 3_656 ?
O3 P1 O4 35.6(3) . 3_656 ?
OH1 P1 O4 89.5(2) . 3_656 ?
O3 P1 O4 41.26(13) 3_656 3_656 ?
K P1 O4 139.53(14) . 3_656 ?
O3 P1 O4 99.95(15) 3_666 3_656 ?
O7 P1 O4 43.45(14) . 3_656 ?
K1 P1 O4 79.08(14) . 3_656 ?
O2 P1 O6 136.2(3) . . ?
O4 P1 O6 104.4(3) . . ?
O3 P1 O6 82.0(2) . . ?
OH1 P1 O6 32.4(3) . . ?
O3 P1 O6 63.90(17) 3_656 . ?
K P1 O6 143.17(14) . . ?
O3 P1 O6 100.00(17) 3_666 . ?
O7 P1 O6 38.57(16) . . ?
K1 P1 O6 133.51(16) . . ?
O4 P1 O6 57.30(15) 3_656 . ?
O7 P2 O8 115.6(4) . 1_545 ?
O7 P2 O6 108.4(4) . . ?
O8 P2 O6 112.1(5) 1_545 . ?
O7 P2 OH5 106.1(5) . . ?
O8 P2 OH5 108.2(4) 1_545 . ?
O6 P2 OH5 105.8(5) . . ?
O7 P2 O4 55.4(3) . 3_656 ?
O8 P2 O4 77.1(3) 1_545 3_656 ?
O6 P2 O4 89.4(3) . 3_656 ?
OH5 P2 O4 159.7(4) . 3_656 ?
O7 P2 OH1 65.6(3) . . ?
O8 P2 OH1 142.0(4) 1_545 . ?
O6 P2 OH1 44.2(3) . . ?
OH5 P2 OH1 107.5(3) . . ?
O4 P2 OH1 74.07(16) 3_656 . ?
O7 P2 OWB 68.4(10) . 3_666 ?
O8 P2 OWB 81.5(6) 1_545 3_666 ?
O6 P2 OWB 165.2(6) . 3_666 ?
OH5 P2 OWB 62.8(9) . 3_666 ?
O4 P2 OWB 99.7(9) 3_656 3_666 ?
OH1 P2 OWB 127.3(7) . 3_666 ?
O7 P2 OWA 96.5(6) . 4_465 ?
O8 P2 OWA 33.4(5) 1_545 4_465 ?
O6 P2 OWA 145.3(5) . 4_465 ?
OH5 P2 OWA 89.4(5) . 4_465 ?
O4 P2 OWA 85.1(5) 3_656 4_465 ?
OH1 P2 OWA 157.9(6) . 4_465 ?
OWB P2 OWA 48.1(8) 3_666 4_465 ?
O7 P2 K2 153.1(3) . 2_645 ?
O8 P2 K2 38.0(3) 1_545 2_645 ?
O6 P2 K2 91.4(3) . 2_645 ?
OH5 P2 K2 84.8(3) . 2_645 ?
O4 P2 K2 108.58(19) 3_656 2_645 ?
OH1 P2 K2 135.44(19) . 2_645 ?
OWB P2 K2 96.7(8) 3_666 2_645 ?
OWA P2 K2 58.5(6) 4_465 2_645 ?
O7 P2 O3 34.9(3) . . ?
O8 P2 O3 119.3(3) 1_545 . ?
O6 P2 O3 75.9(3) . . ?
OH5 P2 O3 128.0(3) . . ?
O4 P2 O3 42.18(15) 3_656 . ?
OH1 P2 O3 39.02(12) . . ?
OWB P2 O3 103.1(9) 3_666 . ?
OWA P2 O3 119.0(6) 4_465 . ?
K2 P2 O3 146.77(18) 2_645 . ?
O7 P2 O2 5.5(3) . 3_666 ?
O8 P2 O2 117.7(3) 1_545 3_666 ?
O6 P2 O2 111.1(3) . 3_666 ?
OH5 P2 O2 100.6(4) . 3_666 ?
O4 P2 O2 60.70(15) 3_656 3_666 ?
OH1 P2 O2 67.44(15) . 3_666 ?
OWB P2 O2 64.6(9) 3_666 3_666 ?
OWA P2 O2 95.9(6) 4_465 3_666 ?
K2 P2 O2 154.02(17) 2_645 3_666 ?
O3 P2 O2 39.29(13) . 3_666 ?
O7 Fe O3 100.5(3) . . ?
O7 Fe O2 88.5(3) . 3_666 ?
O3 Fe O2 92.3(3) . 3_666 ?
O7 Fe O4 93.3(3) . 3_656 ?
O3 Fe O4 90.7(3) . 3_656 ?
O2 Fe O4 176.1(3) 3_666 3_656 ?
O7 Fe O9 168.6(3) . . ?
O3 Fe O9 90.2(2) . . ?
O2 Fe O9 87.3(3) 3_666 . ?
O4 Fe O9 90.2(3) 3_656 . ?
O7 Fe O11 87.7(3) . . ?
O3 Fe O11 171.7(3) . . ?
O2 Fe O11 88.3(3) 3_666 . ?
O4 Fe O11 88.4(3) 3_656 . ?
O9 Fe O11 81.5(2) . . ?
O7 Fe OH1 60.3(2) . . ?
O3 Fe OH1 40.45(19) . . ?
O2 Fe OH1 94.8(2) 3_666 . ?
O4 Fe OH1 89.1(2) 3_656 . ?
O9 Fe OH1 130.7(2) . . ?
O11 Fe OH1 147.7(2) . . ?
O7 Fe O3 84.9(2) . 3_666 ?
O3 Fe O3 56.9(3) . 3_666 ?
O2 Fe O3 37.2(2) 3_666 3_666 ?
O4 Fe O3 146.4(2) 3_656 3_666 ?
O9 Fe O3 98.1(2) . 3_666 ?
O11 Fe O3 125.0(2) . 3_666 ?
OH1 Fe O3 60.92(15) . 3_666 ?
O7 Fe O8 36.7(2) . 1_545 ?
O3 Fe O8 115.6(2) . 1_545 ?
O2 Fe O8 119.4(2) 3_666 1_545 ?
O4 Fe O8 61.2(2) 3_656 1_545 ?
O9 Fe O8 140.0(2) . 1_545 ?
O11 Fe O8 71.0(2) . 1_545 ?
OH1 Fe O8 79.63(17) . 1_545 ?
O3 Fe O8 121.43(15) 3_666 1_545 ?
O7 Fe OH1 126.4(3) . 3_656 ?
O3 Fe OH1 71.1(2) . 3_656 ?
O2 Fe OH1 142.8(2) 3_666 3_656 ?
O4 Fe OH1 36.6(2) 3_656 3_656 ?
O9 Fe OH1 60.6(2) . 3_656 ?
O11 Fe OH1 103.7(2) . 3_656 ?
OH1 Fe OH1 93.11(14) . 3_656 ?
O3 Fe OH1 123.97(14) 3_666 3_656 ?
O8 Fe OH1 97.74(19) 1_545 3_656 ?
O7 Fe O6 32.8(2) . . ?
O3 Fe O6 78.3(2) . . ?
O2 Fe O6 113.1(2) 3_666 . ?
O4 Fe O6 69.9(2) 3_656 . ?
O9 Fe O6 156.6(3) . . ?
O11 Fe O6 109.1(2) . . ?
OH1 Fe O6 40.76(15) . . ?
O3 Fe O6 92.59(16) 3_666 . ?
O8 Fe O6 38.89(18) 1_545 . ?
OH1 Fe O6 96.25(17) 3_656 . ?
O7 Fe O3 91.6(2) . 3_656 ?
O3 Fe O3 56.2(3) . 3_656 ?
O2 Fe O3 148.0(2) 3_666 3_656 ?
O4 Fe O3 35.4(2) 3_656 3_656 ?
O9 Fe O3 97.5(2) . 3_656 ?
O11 Fe O3 123.7(2) . 3_656 ?
OH1 Fe O3 58.34(14) . 3_656 ?
O3 Fe O3 110.95(14) 3_666 3_656 ?
O8 Fe O3 75.66(17) 1_545 3_656 ?
OH1 Fe O3 38.69(13) 3_656 3_656 ?
O6 Fe O3 59.20(15) . 3_656 ?
O10 C1 O9 125.2(8) . . ?
O10 C1 C2 118.5(8) . . ?
O9 C1 C2 116.3(8) . . ?
O10 C1 O2 140.2(7) . 3_666 ?
O9 C1 O2 53.1(5) . 3_666 ?
C2 C1 O2 78.9(6) . 3_666 ?
O10 C1 OH5 49.5(4) . 4_566 ?
O9 C1 OH5 76.2(5) . 4_566 ?
C2 C1 OH5 165.3(7) . 4_566 ?
O2 C1 OH5 115.7(3) 3_666 4_566 ?
O10 C1 O4 144.1(7) . 3_656 ?
O9 C1 O4 51.2(5) . 3_656 ?
C2 C1 O4 77.3(5) . 3_656 ?
O2 C1 O4 71.1(2) 3_666 3_656 ?
OH5 C1 O4 108.0(3) 4_566 3_656 ?
O10 C1 K2 65.9(6) . 3_656 ?
O9 C1 K2 92.5(6) . 3_656 ?
C2 C1 K2 113.1(7) . 3_656 ?
O2 C1 K2 143.8(4) 3_666 3_656 ?
OH5 C1 K2 56.3(2) 4_566 3_656 ?
O4 C1 K2 78.3(3) 3_656 3_656 ?
O10 C1 K 40.1(4) . 1_455 ?
O9 C1 K 164.9(6) . 1_455 ?
C2 C1 K 78.5(5) . 1_455 ?
O2 C1 K 137.9(4) 3_666 1_455 ?
OH5 C1 K 88.8(3) 4_566 1_455 ?
O4 C1 K 135.8(3) 3_656 1_455 ?
K2 C1 K 78.1(2) 3_656 1_455 ?
O10 C1 K2 63.5(6) . 3_666 ?
O9 C1 K2 95.2(6) . 3_666 ?
C2 C1 K2 113.6(7) . 3_666 ?
O2 C1 K2 76.8(3) 3_666 3_666 ?
OH5 C1 K2 70.7(3) 4_566 3_666 ?
O4 C1 K2 143.4(4) 3_656 3_666 ?
K2 C1 K2 122.6(3) 3_656 3_666 ?
K C1 K2 80.4(3) 1_455 3_666 ?
O12 C2 O11 125.5(8) 1_455 . ?
O12 C2 C1 122.1(8) 1_455 . ?
O11 C2 C1 112.4(8) . . ?
O12 C2 O2 144.0(8) 1_455 3_666 ?
O11 C2 O2 53.0(5) . 3_666 ?
C1 C2 O2 73.8(6) . 3_666 ?
O12 C2 O4 141.5(8) 1_455 3_656 ?
O11 C2 O4 50.4(5) . 3_656 ?
C1 C2 O4 76.2(5) . 3_656 ?
O2 C2 O4 70.1(2) 3_666 3_656 ?
O12 C2 K 45.6(4) 1_455 1_455 ?
O11 C2 K 171.1(6) . 1_455 ?
C1 C2 K 76.5(5) . 1_455 ?
O2 C2 K 133.9(3) 3_666 1_455 ?
O4 C2 K 134.1(3) 3_656 1_455 ?
O12 C2 K2 43.5(4) 1_455 1_455 ?
O11 C2 K2 82.0(5) . 1_455 ?
C1 C2 K2 165.5(7) . 1_455 ?
O2 C2 K2 118.8(3) 3_666 1_455 ?
O4 C2 K2 113.8(3) 3_656 1_455 ?
K C2 K2 89.1(3) 1_455 1_455 ?
P1 OH1 O2 35.5(2) . . ?
P1 OH1 O3 34.84(18) . . ?
O2 OH1 O3 60.3(2) . . ?
P1 OH1 O4 34.7(2) . . ?
O2 OH1 O4 58.3(2) . . ?
O3 OH1 O4 60.1(2) . . ?
P1 OH1 O6 128.6(4) . . ?
O2 OH1 O6 157.9(3) . . ?
O3 OH1 O6 98.6(3) . . ?
O4 OH1 O6 119.2(4) . . ?
P1 OH1 K2 126.8(3) . . ?
O2 OH1 K2 103.9(3) . . ?
O3 OH1 K2 161.7(3) . . ?
O4 OH1 K2 104.6(3) . . ?
O6 OH1 K2 97.9(3) . . ?
P1 OH1 N1 112.9(3) . 3_666 ?
O2 OH1 N1 93.2(3) . 3_666 ?
O3 OH1 N1 93.5(3) . 3_666 ?
O4 OH1 N1 147.4(3) . 3_666 ?
O6 OH1 N1 80.8(3) . 3_666 ?
K2 OH1 N1 96.9(3) . 3_666 ?
P1 OH1 O7 94.2(3) . . ?
O2 OH1 O7 109.5(3) . . ?
O3 OH1 O7 59.37(19) . . ?
O4 OH1 O7 113.1(3) . . ?
O6 OH1 O7 49.4(2) . . ?
K2 OH1 O7 138.9(3) . . ?
N1 OH1 O7 58.6(2) 3_666 . ?
P1 OH1 O9 87.9(3) . 3_656 ?
O2 OH1 O9 108.2(3) . 3_656 ?
O3 OH1 O9 100.8(3) . 3_656 ?
O4 OH1 O9 53.9(2) . 3_656 ?
O6 OH1 O9 80.8(3) . 3_656 ?
K2 OH1 O9 74.2(2) . 3_656 ?
N1 OH1 O9 158.2(3) 3_666 3_656 ?
O7 OH1 O9 115.6(3) . 3_656 ?
P1 OH1 O9 85.4(3) . 3_666 ?
O2 OH1 O9 50.9(2) . 3_666 ?
O3 OH1 O9 97.0(3) . 3_666 ?
O4 OH1 O9 106.5(3) . 3_666 ?
O6 OH1 O9 133.6(3) . 3_666 ?
K2 OH1 O9 77.1(2) . 3_666 ?
N1 OH1 O9 54.76(19) 3_666 3_666 ?
O7 OH1 O9 106.3(2) . 3_666 ?
O9 OH1 O9 137.9(3) 3_656 3_666 ?
P1 OH1 P2 115.4(3) . . ?
O2 OH1 P2 135.0(3) . . ?
O3 OH1 P2 81.1(2) . . ?
O4 OH1 P2 122.5(3) . . ?
O6 OH1 P2 24.34(18) . . ?
K2 OH1 P2 117.0(2) . . ?
N1 OH1 P2 65.20(17) 3_666 . ?
O7 OH1 P2 25.50(14) . . ?
O9 OH1 P2 100.6(2) 3_656 . ?
O9 OH1 P2 119.7(2) 3_666 . ?
P1 OH1 Fe 63.5(2) . . ?
O2 OH1 Fe 84.7(2) . . ?
O3 OH1 Fe 28.64(14) . . ?
O4 OH1 Fe 84.7(2) . . ?
O6 OH1 Fe 73.2(2) . . ?
K2 OH1 Fe 169.7(2) . . ?
N1 OH1 Fe 76.77(18) 3_666 . ?
O7 OH1 Fe 30.83(12) . . ?
O9 OH1 Fe 108.8(2) 3_656 . ?
O9 OH1 Fe 105.0(2) 3_666 . ?
P2 OH1 Fe 53.06(11) . . ?
P1 OH1 O3 64.6(2) . 3_656 ?
O2 OH1 O3 99.3(2) . 3_656 ?
O3 OH1 O3 59.1(2) . 3_656 ?
O4 OH1 O3 47.5(2) . 3_656 ?
O6 OH1 O3 72.2(3) . 3_656 ?
K2 OH1 O3 119.5(3) . 3_656 ?
N1 OH1 O3 136.7(2) 3_666 3_656 ?
O7 OH1 O3 78.22(19) . 3_656 ?
O9 OH1 O3 45.47(16) 3_656 3_656 ?
O9 OH1 O3 150.0(2) 3_666 3_656 ?
P2 OH1 O3 77.10(16) . 3_656 ?
Fe OH1 O3 63.51(14) . 3_656 ?
P1 OH1 O3 62.9(3) . 3_666 ?
O2 OH1 O3 46.4(2) . 3_666 ?
O3 OH1 O3 56.4(3) . 3_666 ?
O4 OH1 O3 96.9(2) . 3_666 ?
O6 OH1 O3 117.9(3) . 3_666 ?
K2 OH1 O3 121.0(3) . 3_666 ?
N1 OH1 O3 50.72(18) 3_666 3_666 ?
O7 OH1 O3 71.13(19) . 3_666 ?
O9 OH1 O3 150.7(2) 3_656 3_666 ?
O9 OH1 O3 44.09(16) 3_666 3_666 ?
P2 OH1 O3 94.05(17) . 3_666 ?
Fe OH1 O3 61.19(13) . 3_666 ?
O3 OH1 O3 115.5(2) 3_656 3_666 ?
P1 OH1 Al 58.0(2) . 3_656 ?
O2 OH1 Al 85.0(2) . 3_656 ?
O3 OH1 Al 71.5(2) . 3_656 ?
O4 OH1 Al 26.77(17) . 3_656 ?
O6 OH1 Al 94.8(3) . 3_656 ?
K2 OH1 Al 99.3(2) . 3_656 ?
N1 OH1 Al 163.7(2) 3_666 3_656 ?
O7 OH1 Al 106.7(2) . 3_656 ?
O9 OH1 Al 30.92(12) 3_656 3_656 ?
O9 OH1 Al 131.6(2) 3_666 3_656 ?
P2 OH1 Al 105.03(18) . 3_656 ?
Fe OH1 Al 86.89(14) . 3_656 ?
O3 OH1 Al 28.97(10) 3_656 3_656 ?
O3 OH1 Al 120.51(18) 3_666 3_656 ?
P1 OH1 Al 55.9(2) . 3_666 ?
O2 OH1 Al 24.77(18) . 3_666 ?
O3 OH1 Al 68.6(2) . 3_666 ?
O4 OH1 Al 82.9(2) . 3_666 ?
O6 OH1 Al 145.7(3) . 3_666 ?
K2 OH1 Al 101.2(2) . 3_666 ?
N1 OH1 Al 68.90(19) 3_666 3_666 ?
O7 OH1 Al 99.3(2) . 3_666 ?
O9 OH1 Al 131.8(2) 3_656 3_666 ?
O9 OH1 Al 30.31(12) 3_666 3_666 ?
P2 OH1 Al 122.28(19) . 3_666 ?
Fe OH1 Al 84.23(14) . 3_666 ?
O3 OH1 Al 120.24(18) 3_656 3_666 ?
O3 OH1 Al 28.33(10) 3_666 3_666 ?
Al OH1 Al 109.69(16) 3_656 3_666 ?
P1 OH1 O4 67.6(2) . 3_656 ?
O2 OH1 O4 99.4(2) . 3_656 ?
O3 OH1 O4 39.90(19) . 3_656 ?
O4 OH1 O4 73.0(2) . 3_656 ?
O6 OH1 O4 61.1(2) . 3_656 ?
K2 OH1 O4 150.5(3) . 3_656 ?
N1 OH1 O4 99.5(2) 3_666 3_656 ?
O7 OH1 O4 42.22(16) . 3_656 ?
O9 OH1 O4 81.68(19) 3_656 3_656 ?
O9 OH1 O4 132.3(2) 3_666 3_656 ?
P2 OH1 O4 51.10(13) . 3_656 ?
Fe OH1 O4 27.90(11) . 3_656 ?
O3 OH1 O4 37.71(13) 3_656 3_656 ?
O3 OH1 O4 88.19(17) 3_666 3_656 ?
Al OH1 O4 64.92(14) 3_656 3_656 ?
Al OH1 O4 107.45(17) 3_666 3_656 ?
P1 OH1 OH5 136.6(3) . 2_645 ?
O2 OH1 OH5 145.2(3) . 2_645 ?
O3 OH1 OH5 138.8(3) . 2_645 ?
O4 OH1 OH5 102.2(3) . 2_645 ?
O6 OH1 OH5 55.3(2) . 2_645 ?
K2 OH1 OH5 49.6(2) . 2_645 ?
N1 OH1 OH5 110.3(2) 3_666 2_645 ?
O7 OH1 OH5 104.7(2) . 2_645 ?
O9 OH1 OH5 48.70(17) 3_656 2_645 ?
O9 OH1 OH5 124.2(2) 3_666 2_645 ?
P2 OH1 OH5 79.40(17) . 2_645 ?
Fe OH1 OH5 124.6(2) . 2_645 ?
O3 OH1 OH5 81.2(2) 3_656 2_645 ?
O3 OH1 OH5 160.4(2) 3_666 2_645 ?
Al OH1 OH5 79.06(19) 3_656 2_645 ?
Al OH1 OH5 150.9(2) 3_666 2_645 ?
O4 OH1 OH5 101.4(2) 3_656 2_645 ?
P1 O2 Al 143.1(4) . 3_666 ?
P1 O2 O4 36.5(2) . . ?
Al O2 O4 174.2(4) 3_666 . ?
P1 O2 OH1 37.3(2) . . ?
Al O2 OH1 121.9(3) 3_666 . ?
O4 O2 OH1 61.5(3) . . ?
P1 O2 O3 34.0(2) . . ?
Al O2 O3 115.6(3) 3_666 . ?
O4 O2 O3 61.2(3) . . ?
OH1 O2 O3 60.4(2) . . ?
P1 O2 O7 135.4(4) . 3_666 ?
Al O2 O7 45.1(2) 3_666 3_666 ?
O4 O2 O7 129.7(3) . 3_666 ?
OH1 O2 O7 155.5(3) . 3_666 ?
O3 O2 O7 103.5(3) . 3_666 ?
P1 O2 O9 118.1(3) . 3_666 ?
Al O2 O9 47.0(2) 3_666 3_666 ?
O4 O2 O9 138.5(3) . 3_666 ?
OH1 O2 O9 82.3(3) . 3_666 ?
O3 O2 O9 119.2(3) . 3_666 ?
O7 O2 O9 91.6(3) 3_666 3_666 ?
P1 O2 K 99.4(3) . . ?
Al O2 K 117.1(3) 3_666 . ?
O4 O2 K 63.0(2) . . ?
OH1 O2 K 112.3(3) . . ?
O3 O2 K 117.5(3) . . ?
O7 O2 K 91.3(2) 3_666 . ?
O9 O2 K 120.6(3) 3_666 . ?
P1 O2 O11 164.1(4) . 3_666 ?
Al O2 O11 47.2(2) 3_666 3_666 ?
O4 O2 O11 135.1(4) . 3_666 ?
OH1 O2 O11 131.3(3) . 3_666 ?
O3 O2 O11 161.5(3) . 3_666 ?
O7 O2 O11 60.0(2) 3_666 3_666 ?
O9 O2 O11 57.2(2) 3_666 3_666 ?
K O2 O11 73.9(2) . 3_666 ?
P1 O2 O3 100.2(3) . 3_666 ?
Al O2 O3 43.28(19) 3_666 3_666 ?
O4 O2 O3 134.7(4) . 3_666 ?
OH1 O2 O3 91.9(3) . 3_666 ?
O3 O2 O3 74.0(3) . 3_666 ?
O7 O2 O3 64.8(2) 3_666 3_666 ?
O9 O2 O3 60.3(2) 3_666 3_666 ?
K O2 O3 155.9(3) . 3_666 ?
O11 O2 O3 90.2(3) 3_666 3_666 ?
P1 O2 C1 124.0(4) . 3_666 ?
Al O2 C1 57.6(3) 3_666 3_666 ?
O4 O2 C1 128.1(3) . 3_666 ?
OH1 O2 C1 86.9(3) . 3_666 ?
O3 O2 C1 137.6(3) . 3_666 ?
O7 O2 C1 96.4(3) 3_666 3_666 ?
O9 O2 C1 22.1(2) 3_666 3_666 ?
K O2 C1 98.9(3) . 3_666 ?
O11 O2 C1 45.5(2) 3_666 3_666 ?
O3 O2 C1 81.6(3) 3_666 3_666 ?
P1 O2 C2 143.2(4) . 3_666 ?
Al O2 C2 57.7(3) 3_666 3_666 ?
O4 O2 C2 126.7(4) . 3_666 ?
OH1 O2 C2 109.8(3) . 3_666 ?
O3 O2 C2 164.6(3) . 3_666 ?
O7 O2 C2 81.4(3) 3_666 3_666 ?
O9 O2 C2 45.5(2) 3_666 3_666 ?
K O2 C2 76.6(2) . 3_666 ?
O11 O2 C2 22.0(2) 3_666 3_666 ?
O3 O2 C2 95.6(3) 3_666 3_666 ?
C1 O2 C2 27.3(2) 3_666 3_666 ?
P1 O2 K1 80.9(3) . . ?
Al O2 K1 93.3(2) 3_666 . ?
O4 O2 K1 80.9(3) . . ?
OH1 O2 K1 114.8(3) . . ?
O3 O2 K1 55.0(2) . . ?
O7 O2 K1 55.6(2) 3_666 . ?
O9 O2 K1 136.3(3) 3_666 . ?
K O2 K1 90.9(2) . . ?
O11 O2 K1 113.2(3) 3_666 . ?
O3 O2 K1 78.5(2) 3_666 . ?
C1 O2 K1 150.7(3) 3_666 . ?
C2 O2 K1 135.1(3) 3_666 . ?
P1 O2 O12 94.0(3) . . ?
Al O2 O12 112.1(3) 3_666 . ?
O4 O2 O12 72.7(3) . . ?
OH1 O2 O12 77.8(2) . . ?
O3 O2 O12 128.0(3) . . ?
O7 O2 O12 124.8(3) 3_666 . ?
O9 O2 O12 80.7(2) 3_666 . ?
K O2 O12 50.74(16) . . ?
O11 O2 O12 70.5(2) 3_666 . ?
O3 O2 O12 140.7(3) 3_666 . ?
C1 O2 O12 60.4(3) 3_666 . ?
C2 O2 O12 54.7(2) 3_666 . ?
K1 O2 O12 140.3(2) . . ?
P1 O2 O4 144.4(4) . 1_565 ?
Al O2 O4 1.95(13) 3_666 1_565 ?
O4 O2 O4 175.7(4) . 1_565 ?
OH1 O2 O4 121.8(3) . 1_565 ?
O3 O2 O4 117.4(3) . 1_565 ?
O7 O2 O4 46.1(2) 3_666 1_565 ?
O9 O2 O4 45.79(19) 3_666 1_565 ?
K O2 O4 116.1(2) . 1_565 ?
O11 O2 O4 45.58(19) 3_666 1_565 ?
O3 O2 O4 44.80(18) 3_666 1_565 ?
C1 O2 O4 55.9(2) 3_666 1_565 ?
C2 O2 O4 55.7(2) 3_666 1_565 ?
K1 O2 O4 95.0(2) . 1_565 ?
O12 O2 O4 110.2(2) . 1_565 ?
P1 O2 P1 88.6(3) . 3_666 ?
Al O2 P1 57.08(17) 3_666 3_666 ?
O4 O2 P1 119.7(3) . 3_666 ?
OH1 O2 P1 90.7(2) . 3_666 ?
O3 O2 P1 58.6(2) . 3_666 ?
O7 O2 P1 64.77(19) 3_666 3_666 ?
O9 O2 P1 77.6(2) 3_666 3_666 ?
K O2 P1 151.4(2) . 3_666 ?
O11 O2 P1 104.1(2) 3_666 3_666 ?
O3 O2 P1 17.71(14) 3_666 3_666 ?
C1 O2 P1 99.1(2) 3_666 3_666 ?
C2 O2 P1 112.5(3) 3_666 3_666 ?
K1 O2 P1 63.12(15) . 3_666 ?
O12 O2 P1 156.6(2) . 3_666 ?
O4 O2 P1 58.85(15) 1_565 3_666 ?
P1 O2 P2 134.1(3) . 3_666 ?
Al O2 P2 48.13(16) 3_666 3_666 ?
O4 O2 P2 126.8(3) . 3_666 ?
OH1 O2 P2 157.2(3) . 3_666 ?
O3 O2 P2 103.0(2) . 3_666 ?
O7 O2 P2 3.11(16) 3_666 3_666 ?
O9 O2 P2 94.5(2) 3_666 3_666 ?
K O2 P2 88.85(18) . 3_666 ?
O11 O2 P2 61.10(18) 3_666 3_666 ?
O3 O2 P2 67.37(18) 3_666 3_666 ?
C1 O2 P2 98.7(2) 3_666 3_666 ?
C2 O2 P2 82.7(2) 3_666 3_666 ?
K1 O2 P2 53.74(15) . 3_666 ?
O12 O2 P2 124.2(2) . 3_666 ?
O4 O2 P2 49.07(13) 1_565 3_666 ?
P1 O2 P2 66.60(12) 3_666 3_666 ?
P1 O2 OWB 128.4(7) . . ?
Al O2 OWB 83.9(7) 3_666 . ?
O4 O2 OWB 94.3(7) . . ?
OH1 O2 OWB 149.6(6) . . ?
O3 O2 OWB 126.3(5) . . ?
O7 O2 OWB 54.4(6) 3_666 . ?
O9 O2 OWB 110.5(6) 3_666 . ?
K O2 OWB 37.3(6) . . ?
O11 O2 OWB 53.3(6) 3_666 . ?
O3 O2 OWB 118.5(6) 3_666 . ?
C1 O2 OWB 95.8(6) 3_666 . ?
C2 O2 OWB 68.5(5) 3_666 . ?
K1 O2 OWB 75.6(5) . . ?
O12 O2 OWB 77.3(5) . . ?
O4 O2 OWB 83.4(6) 1_565 . ?
P1 O2 OWB 118.5(5) 3_666 . ?
P2 O2 OWB 52.3(5) 3_666 . ?
P1 O3 Fe 147.4(4) . . ?
P1 O3 O2 33.9(2) . . ?
Fe O3 O2 147.6(4) . . ?
P1 O3 OH1 36.5(2) . . ?
Fe O3 OH1 110.9(3) . . ?
O2 O3 OH1 59.3(2) . . ?
P1 O3 O4 33.8(2) . . ?
Fe O3 O4 148.3(4) . . ?
O2 O3 O4 58.0(2) . . ?
OH1 O3 O4 60.1(2) . . ?
P1 O3 O4 125.1(4) . 3_656 ?
Fe O3 O4 45.3(2) . 3_656 ?
O2 O3 O4 159.0(3) . 3_656 ?
OH1 O3 O4 103.0(3) . 3_656 ?
O4 O3 O4 104.5(3) . 3_656 ?
P1 O3 O9 166.4(3) . . ?
Fe O3 O9 46.13(18) . . ?
O2 O3 O9 139.4(3) . . ?
OH1 O3 O9 157.0(3) . . ?
O4 O3 O9 136.7(3) . . ?
O4 O3 O9 60.9(2) 3_656 . ?
P1 O3 O2 129.4(4) . 3_666 ?
Fe O3 O2 44.4(2) . 3_666 ?
O2 O3 O2 106.0(3) . 3_666 ?
OH1 O3 O2 108.0(3) . 3_666 ?
O4 O3 O2 162.9(3) . 3_666 ?
O4 O3 O2 89.7(2) 3_656 3_666 ?
O9 O3 O2 58.8(2) . 3_666 ?
P1 O3 O7 107.8(3) . . ?
Fe O3 O7 39.71(17) . . ?
O2 O3 O7 118.4(3) . . ?
OH1 O3 O7 71.4(2) . . ?
O4 O3 O7 123.5(3) . . ?
O4 O3 O7 59.1(2) 3_656 . ?
O9 O3 O7 85.8(2) . . ?
O2 O3 O7 56.1(2) 3_666 . ?
P1 O3 K1 104.6(3) . . ?
Fe O3 K1 107.2(2) . . ?
O2 O3 K1 81.0(2) . . ?
OH1 O3 K1 139.5(3) . . ?
O4 O3 K1 93.2(2) . . ?
O4 O3 K1 113.6(3) 3_656 . ?
O9 O3 K1 62.82(19) . . ?
O2 O3 K1 89.7(2) 3_666 . ?
O7 O3 K1 143.2(3) . . ?
P1 O3 O3 83.3(3) . 3_666 ?
Fe O3 O3 93.4(3) . 3_666 ?
O2 O3 O3 55.9(2) . 3_666 ?
OH1 O3 O3 81.8(3) . 3_666 ?
O4 O3 O3 113.5(3) . 3_666 ?
O4 O3 O3 137.9(3) 3_656 3_666 ?
O9 O3 O3 99.2(3) . 3_666 ?
O2 O3 O3 50.2(2) 3_666 3_666 ?
O7 O3 O3 84.3(3) . 3_666 ?
K1 O3 O3 82.5(3) . 3_666 ?
P1 O3 O3 80.0(3) . 3_656 ?
Fe O3 O3 94.7(3) . 3_656 ?
O2 O3 O3 111.4(3) . 3_656 ?
OH1 O3 O3 78.1(3) . 3_656 ?
O4 O3 O3 54.5(2) . 3_656 ?
O4 O3 O3 50.0(2) 3_656 3_656 ?
O9 O3 O3 99.7(3) . 3_656 ?
O2 O3 O3 138.8(3) 3_666 3_656 ?
O7 O3 O3 90.4(3) . 3_656 ?
K1 O3 O3 112.3(3) . 3_656 ?
O3 O3 O3 159.9(4) 3_666 3_656 ?
P1 O3 P1 107.1(3) . 3_656 ?
Fe O3 P1 72.0(2) . 3_656 ?
O2 O3 P1 137.6(3) . 3_656 ?
OH1 O3 P1 99.9(2) . 3_656 ?
O4 O3 P1 79.6(3) . 3_656 ?
O4 O3 P1 27.16(15) 3_656 3_656 ?
O9 O3 P1 73.3(2) . 3_656 ?
O2 O3 P1 115.9(2) 3_666 3_656 ?
O7 O3 P1 82.2(2) . 3_656 ?
K1 O3 P1 104.6(2) . 3_656 ?
O3 O3 P1 165.0(3) 3_666 3_656 ?
O3 O3 P1 27.10(13) 3_656 3_656 ?
P1 O3 P1 110.2(3) . 3_666 ?
Fe O3 P1 70.9(2) . 3_666 ?
O2 O3 P1 81.3(2) . 3_666 ?
OH1 O3 P1 103.4(3) . 3_666 ?
O4 O3 P1 139.1(3) . 3_666 ?
O4 O3 P1 116.0(2) 3_656 3_666 ?
O9 O3 P1 73.0(2) . 3_666 ?
O2 O3 P1 26.56(15) 3_666 3_666 ?
O7 O3 P1 76.5(2) . 3_666 ?
K1 O3 P1 76.26(19) . 3_666 ?
O3 O3 P1 26.92(13) 3_666 3_666 ?
O3 O3 P1 165.2(3) 3_656 3_666 ?
P1 O3 P1 141.17(17) 3_656 3_666 ?
P1 O3 OH1 113.9(3) . 3_656 ?
Fe O3 OH1 79.9(2) . 3_656 ?
O2 O3 OH1 132.3(3) . 3_656 ?
OH1 O3 OH1 120.9(2) . 3_656 ?
O4 O3 OH1 80.5(3) . 3_656 ?
O4 O3 OH1 43.97(18) 3_656 3_656 ?
O9 O3 OH1 60.6(2) . 3_656 ?
O2 O3 OH1 116.5(2) 3_666 3_656 ?
O7 O3 OH1 103.1(2) . 3_656 ?
K1 O3 OH1 78.8(2) . 3_656 ?
O3 O3 OH1 157.3(3) 3_666 3_656 ?
O3 O3 OH1 42.71(19) 3_656 3_656 ?
P1 O3 OH1 25.77(12) 3_656 3_656 ?
P1 O3 OH1 133.42(18) 3_666 3_656 ?
P1 O3 OH1 116.3(3) . 3_666 ?
Fe O3 OH1 79.1(2) . 3_666 ?
O2 O3 OH1 82.6(3) . 3_666 ?
OH1 O3 OH1 123.6(3) . 3_666 ?
O4 O3 OH1 132.2(3) . 3_666 ?
O4 O3 OH1 118.2(2) 3_656 3_666 ?
O9 O3 OH1 61.0(2) . 3_666 ?
O2 O3 OH1 41.72(18) 3_666 3_666 ?
O7 O3 OH1 97.5(2) . 3_666 ?
K1 O3 OH1 51.62(18) . 3_666 ?
O3 O3 OH1 41.78(18) 3_666 3_666 ?
O3 O3 OH1 158.2(3) 3_656 3_666 ?
P1 O3 OH1 134.16(18) 3_656 3_666 ?
P1 O3 OH1 24.96(11) 3_666 3_666 ?
OH1 O3 OH1 115.5(2) 3_656 3_666 ?
P1 O3 Al 58.9(2) . 3_666 ?
Fe O3 Al 123.1(3) . 3_666 ?
O2 O3 Al 27.16(18) . 3_666 ?
OH1 O3 Al 72.8(2) . 3_666 ?
O4 O3 Al 85.0(2) . 3_666 ?
O4 O3 Al 166.2(2) 3_656 3_666 ?
O9 O3 Al 118.6(3) . 3_666 ?
O2 O3 Al 79.4(2) 3_666 3_666 ?
O7 O3 Al 107.3(2) . 3_666 ?
K1 O3 Al 75.20(18) . 3_666 ?
O3 O3 Al 29.67(13) 3_666 3_666 ?
O3 O3 Al 138.4(2) 3_656 3_666 ?
P1 O3 Al 164.62(18) 3_656 3_666 ?
P1 O3 Al 54.14(13) 3_666 3_666 ?
OH1 O3 Al 149.43(19) 3_656 3_666 ?
OH1 O3 Al 57.89(15) 3_666 3_666 ?
P1 O3 O6 96.6(3) . 3_656 ?
Fe O3 O6 111.0(3) . 3_656 ?
O2 O3 O6 97.0(2) . 3_656 ?
OH1 O3 O6 126.8(3) . 3_656 ?
O4 O3 O6 66.9(2) . 3_656 ?
O4 O3 O6 84.7(2) 3_656 3_656 ?
O9 O3 O6 71.0(2) . 3_656 ?
O2 O3 O6 124.9(2) 3_666 3_656 ?
O7 O3 O6 143.5(3) . 3_656 ?
K1 O3 O6 45.2(2) . 3_656 ?
O3 O3 O6 126.2(3) 3_666 3_656 ?
O3 O3 O6 67.2(2) 3_656 3_656 ?
P1 O3 O6 64.51(18) 3_656 3_656 ?
P1 O3 O6 120.3(2) 3_666 3_656 ?
OH1 O3 O6 40.95(17) 3_656 3_656 ?
OH1 O3 O6 95.4(2) 3_666 3_656 ?
Al O3 O6 108.51(19) 3_666 3_656 ?
P1 O4 Al 141.5(4) . 3_656 ?
P1 O4 O2 36.3(2) . . ?
Al O4 O2 176.7(4) 3_656 . ?
P1 O4 O3 33.8(2) . . ?
Al O4 O3 118.6(3) 3_656 . ?
O2 O4 O3 60.9(3) . . ?
P1 O4 OH1 36.3(2) . . ?
Al O4 OH1 116.6(3) 3_656 . ?
O2 O4 OH1 60.2(3) . . ?
O3 O4 OH1 59.9(2) . . ?
P1 O4 O3 99.2(3) . 3_656 ?
Al O4 O3 43.98(19) 3_656 3_656 ?
O2 O4 O3 134.7(4) . 3_656 ?
O3 O4 O3 75.5(3) . 3_656 ?
OH1 O4 O3 88.6(3) . 3_656 ?
P1 O4 K 99.3(3) . . ?
Al O4 K 118.9(3) 3_656 . ?
O2 O4 K 63.0(2) . . ?
O3 O4 K 117.2(3) . . ?
OH1 O4 K 111.2(3) . . ?
O3 O4 K 159.8(3) 3_656 . ?
P1 O4 O11 158.6(4) . 3_656 ?
Al O4 O11 47.1(2) 3_656 3_656 ?
O2 O4 O11 133.6(4) . 3_656 ?
O3 O4 O11 165.3(3) . 3_656 ?
OH1 O4 O11 126.1(3) . 3_656 ?
O3 O4 O11 90.8(3) 3_656 3_656 ?
K O4 O11 74.6(2) . 3_656 ?
P1 O4 O9 113.0(3) . 3_656 ?
Al O4 O9 45.5(2) 3_656 3_656 ?
O2 O4 O9 131.5(3) . 3_656 ?
O3 O4 O9 118.3(3) . 3_656 ?
OH1 O4 O9 77.7(3) . 3_656 ?
O3 O4 O9 59.8(2) 3_656 3_656 ?
K O4 O9 119.0(3) . 3_656 ?
O11 O4 O9 56.3(2) 3_656 3_656 ?
P1 O4 O7 142.8(4) . 3_656 ?
Al O4 O7 42.7(2) 3_656 3_656 ?
O2 O4 O7 140.5(3) . 3_656 ?
O3 O4 O7 109.4(3) . 3_656 ?
OH1 O4 O7 152.3(3) . 3_656 ?
O3 O4 O7 63.7(2) 3_656 3_656 ?
K O4 O7 96.4(2) . 3_656 ?
O11 O4 O7 58.6(2) 3_656 3_656 ?
O9 O4 O7 87.7(3) 3_656 3_656 ?
P1 O4 P2 125.5(3) . 3_656 ?
Al O4 P2 69.3(2) 3_656 3_656 ?
O2 O4 P2 113.9(3) . 3_656 ?
O3 O4 P2 98.1(2) . 3_656 ?
OH1 O4 P2 157.7(3) . 3_656 ?
O3 O4 P2 82.2(2) 3_656 3_656 ?
K O4 P2 80.56(18) . 3_656 ?
O11 O4 P2 74.4(2) 3_656 3_656 ?
O9 O4 P2 114.0(3) 3_656 3_656 ?
O7 O4 P2 26.60(16) 3_656 3_656 ?
P1 O4 O8 119.9(4) . 3_666 ?
Al O4 O8 88.4(3) 3_656 3_666 ?
O2 O4 O8 94.8(3) . 3_666 ?
O3 O4 O8 105.3(3) . 3_666 ?
OH1 O4 O8 154.6(3) . 3_666 ?
O3 O4 O8 108.5(3) 3_656 3_666 ?
K O4 O8 54.53(18) . 3_666 ?
O11 O4 O8 73.8(2) 3_656 3_666 ?
O9 O4 O8 127.0(3) 3_656 3_666 ?
O7 O4 O8 48.5(2) 3_656 3_666 ?
P2 O4 O8 26.35(15) 3_656 3_666 ?
P1 O4 C1 119.1(4) . 3_656 ?
Al O4 C1 54.7(2) 3_656 3_656 ?
O2 O4 C1 123.0(3) . 3_656 ?
O3 O4 C1 135.4(3) . 3_656 ?
OH1 O4 C1 83.2(3) . 3_656 ?
O3 O4 C1 79.8(3) 3_656 3_656 ?
K O4 C1 98.1(3) . 3_656 ?
O11 O4 C1 44.0(2) 3_656 3_656 ?
O9 O4 C1 20.91(19) 3_656 3_656 ?
O7 O4 C1 91.5(3) 3_656 3_656 ?
P2 O4 C1 114.7(3) 3_656 3_656 ?
O8 O4 C1 117.7(3) 3_666 3_656 ?
P1 O4 C2 137.9(4) . 3_656 ?
Al O4 C2 56.1(2) 3_656 3_656 ?
O2 O4 C2 123.3(4) . 3_656 ?
O3 O4 C2 161.9(3) . 3_656 ?
OH1 O4 C2 105.4(3) . 3_656 ?
O3 O4 C2 94.7(3) 3_656 3_656 ?
K O4 C2 76.7(2) . 3_656 ?
O11 O4 C2 21.1(2) 3_656 3_656 ?
O9 O4 C2 44.5(2) 3_656 3_656 ?
O7 O4 C2 78.6(3) 3_656 3_656 ?
P2 O4 C2 95.5(2) 3_656 3_656 ?
O8 O4 C2 92.2(3) 3_666 3_656 ?
C1 O4 C2 26.5(2) 3_656 3_656 ?
P1 O4 O6 102.6(3) . 3_656 ?
Al O4 O6 80.4(2) 3_656 3_656 ?
O2 O4 O6 102.3(3) . 3_656 ?
O3 O4 O6 73.1(2) . 3_656 ?
OH1 O4 O6 132.7(3) . 3_656 ?
O3 O4 O6 74.3(2) 3_656 3_656 ?
K O4 O6 93.9(2) . 3_656 ?
O11 O4 O6 98.4(2) 3_656 3_656 ?
O9 O4 O6 124.7(3) 3_656 3_656 ?
O7 O4 O6 42.6(2) 3_656 3_656 ?
P2 O4 O6 25.05(14) 3_656 3_656 ?
O8 O4 O6 42.4(2) 3_666 3_656 ?
C1 O4 O6 133.7(3) 3_656 3_656 ?
C2 O4 O6 119.4(3) 3_656 3_656 ?
P1 O4 P1 87.7(3) . 3_656 ?
Al O4 P1 59.56(18) 3_656 3_656 ?
O2 O4 P1 120.0(3) . 3_656 ?
O3 O4 P1 59.1(2) . 3_656 ?
OH1 O4 P1 88.3(2) . 3_656 ?
O3 O4 P1 19.28(13) 3_656 3_656 ?
K O4 P1 155.5(2) . 3_656 ?
O11 O4 P1 106.4(2) 3_656 3_656 ?
O9 O4 P1 78.6(2) 3_656 3_656 ?
O7 O4 P1 65.58(18) 3_656 3_656 ?
P2 O4 P1 76.30(14) 3_656 3_656 ?
O8 O4 P1 101.6(2) 3_666 3_656 ?
C1 O4 P1 98.9(2) 3_656 3_656 ?
C2 O4 P1 113.4(3) 3_656 3_656 ?
O6 O4 P1 61.62(16) 3_656 3_656 ?
P1 O4 O2 142.4(4) . 1_545 ?
Al O4 O2 1.94(13) 3_656 1_545 ?
O2 O4 O2 175.7(4) . 1_545 ?
O3 O4 O2 120.4(3) . 1_545 ?
OH1 O4 O2 116.4(3) . 1_545 ?
O3 O4 O2 45.49(18) 3_656 1_545 ?
K O4 O2 117.8(2) . 1_545 ?
O11 O4 O2 45.43(19) 3_656 1_545 ?
O9 O4 O2 44.27(19) 3_656 1_545 ?
O7 O4 O2 43.64(19) 3_656 1_545 ?
P2 O4 O2 70.23(16) 3_656 1_545 ?
O8 O4 O2 88.8(2) 3_666 1_545 ?
C1 O4 O2 53.0(2) 3_656 1_545 ?
C2 O4 O2 54.1(2) 3_656 1_545 ?
O6 O4 O2 82.0(2) 3_656 1_545 ?
P1 O4 O2 61.32(15) 3_656 1_545 ?
P1 O4 K1 66.0(2) . . ?
Al O4 K1 120.4(3) 3_656 . ?
O2 O4 K1 62.0(2) . . ?
O3 O4 K1 47.76(18) . . ?
OH1 O4 K1 101.8(2) . . ?
O3 O4 K1 98.0(2) 3_656 . ?
K O4 K1 82.30(19) . . ?
O11 O4 K1 131.5(2) 3_656 . ?
O9 O4 K1 157.7(3) 3_656 . ?
O7 O4 K1 83.1(2) 3_656 . ?
P2 O4 K1 59.94(15) 3_656 . ?
O8 O4 K1 58.2(2) 3_666 . ?
C1 O4 K1 174.6(3) 3_656 . ?
C2 O4 K1 150.2(3) 3_656 . ?
O6 O4 K1 40.94(17) 3_656 . ?
P1 O4 K1 79.15(15) 3_656 . ?
O2 O4 K1 122.1(2) 1_545 . ?
P1 O4 OH1 95.2(3) . 3_656 ?
Al O4 OH1 63.0(2) 3_656 3_656 ?
O2 O4 OH1 118.0(3) . 3_656 ?
O3 O4 OH1 61.7(2) . 3_656 ?
OH1 O4 OH1 107.0(2) . 3_656 ?
O3 O4 OH1 37.08(16) 3_656 3_656 ?
K O4 OH1 132.6(2) . 3_656 ?
O11 O4 OH1 104.1(2) 3_656 3_656 ?
O9 O4 OH1 95.5(2) 3_656 3_656 ?
O7 O4 OH1 50.63(18) 3_656 3_656 ?
P2 O4 OH1 54.82(13) 3_656 3_656 ?
O8 O4 OH1 79.2(2) 3_666 3_656 ?
C1 O4 OH1 113.5(3) 3_656 3_656 ?
C2 O4 OH1 118.6(3) 3_656 3_656 ?
O6 O4 OH1 38.82(16) 3_656 3_656 ?
P1 O4 OH1 22.85(10) 3_656 3_656 ?
O2 O4 OH1 64.93(18) 1_545 3_656 ?
K1 O4 OH1 63.11(16) . 3_656 ?
P2 OH5 O7 35.9(3) . . ?
P2 OH5 O6 36.7(3) . . ?
O7 OH5 O6 59.9(3) . . ?
P2 OH5 O8 35.1(3) . 1_545 ?
O7 OH5 O8 61.9(3) . 1_545 ?
O6 OH5 O8 61.1(3) . 1_545 ?
P2 OH5 O10 119.6(4) . 4_565 ?
O7 OH5 O10 134.6(4) . 4_565 ?
O6 OH5 O10 130.1(4) . 4_565 ?
O8 OH5 O10 84.5(3) 1_545 4_565 ?
P2 OH5 N1 89.9(3) . 3_666 ?
O7 OH5 N1 64.0(2) . 3_666 ?
O6 OH5 N1 79.9(3) . 3_666 ?
O8 OH5 N1 123.9(3) 1_545 3_666 ?
O10 OH5 N1 148.5(4) 4_565 3_666 ?
P2 OH5 N1 97.4(4) . 4_565 ?
O7 OH5 N1 120.0(3) . 4_565 ?
O6 OH5 N1 62.6(3) . 4_565 ?
O8 OH5 N1 103.4(4) 1_545 4_565 ?
O10 OH5 N1 95.7(3) 4_565 4_565 ?
N1 OH5 N1 90.9(2) 3_666 4_565 ?
P2 OH5 O9 134.1(5) . 4_565 ?
O7 OH5 O9 170.0(4) . 4_565 ?
O6 OH5 O9 112.7(4) . 4_565 ?
O8 OH5 O9 109.2(3) 1_545 4_565 ?
O10 OH5 O9 43.6(2) 4_565 4_565 ?
N1 OH5 O9 123.1(3) 3_666 4_565 ?
N1 OH5 O9 55.8(2) 4_565 4_565 ?
P2 OH5 N2 149.5(5) . 2_655 ?
O7 OH5 N2 116.8(4) . 2_655 ?
O6 OH5 N2 162.0(4) . 2_655 ?
O8 OH5 N2 135.1(4) 1_545 2_655 ?
O10 OH5 N2 66.0(3) 4_565 2_655 ?
N1 OH5 N2 83.0(3) 3_666 2_655 ?
N1 OH5 N2 112.2(3) 4_565 2_655 ?
O9 OH5 N2 72.3(2) 4_565 2_655 ?
P2 OH5 C1 131.2(5) . 4_565 ?
O7 OH5 C1 155.4(4) . 4_565 ?
O6 OH5 C1 125.4(4) . 4_565 ?
O8 OH5 C1 98.2(3) 1_545 4_565 ?
O10 OH5 C1 21.3(2) 4_565 4_565 ?
N1 OH5 C1 137.9(3) 3_666 4_565 ?
N1 OH5 C1 76.7(3) 4_565 4_565 ?
O9 OH5 C1 22.41(19) 4_565 4_565 ?
N2 OH5 C1 65.8(3) 2_655 4_565 ?
P2 OH5 OWB 91.8(12) . 3_666 ?
O7 OH5 OWB 71.7(13) . 3_666 ?
O6 OH5 OWB 127.8(13) . 3_666 ?
O8 OH5 OWB 80.1(8) 1_545 3_666 ?
O10 OH5 OWB 73.3(12) 4_565 3_666 ?
N1 OH5 OWB 96.6(8) 3_666 3_666 ?
N1 OH5 OWB 168.2(13) 4_565 3_666 ?
O9 OH5 OWB 112.4(13) 4_565 3_666 ?
N2 OH5 OWB 59.9(11) 2_655 3_666 ?
C1 OH5 OWB 91.6(13) 4_565 3_666 ?
P2 OH5 O6 121.0(4) . 2_655 ?
O7 OH5 O6 113.5(3) . 2_655 ?
O6 OH5 O6 87.6(3) . 2_655 ?
O8 OH5 O6 146.8(4) 1_545 2_655 ?
O10 OH5 O6 111.2(3) 4_565 2_655 ?
N1 OH5 O6 53.6(2) 3_666 2_655 ?
N1 OH5 O6 48.0(2) 4_565 2_655 ?
O9 OH5 O6 71.1(2) 4_565 2_655 ?
N2 OH5 O6 77.6(3) 2_655 2_655 ?
C1 OH5 O6 91.1(3) 4_565 2_655 ?
OWB OH5 O6 131.6(7) 3_666 2_655 ?
P2 OH5 OWA 100.3(7) . 3_666 ?
O7 OH5 OWA 81.5(8) . 3_666 ?
O6 OH5 OWA 136.7(7) . 3_666 ?
O8 OH5 OWA 84.6(5) 1_545 3_666 ?
O10 OH5 OWA 64.8(7) 4_565 3_666 ?
N1 OH5 OWA 101.4(5) 3_666 3_666 ?
N1 OH5 OWA 158.4(7) 4_565 3_666 ?
O9 OH5 OWA 102.7(7) 4_565 3_666 ?
N2 OH5 OWA 52.9(6) 2_655 3_666 ?
C1 OH5 OWA 82.3(7) 4_565 3_666 ?
OWB OH5 OWA 9.8(8) 3_666 3_666 ?
O6 OH5 OWA 128.3(5) 2_655 3_666 ?
P2 OH5 K2 72.2(3) . 2_645 ?
O7 OH5 K2 105.0(3) . 2_645 ?
O6 OH5 K2 75.8(3) . 2_645 ?
O8 OH5 K2 43.7(2) 1_545 2_645 ?
O10 OH5 K2 54.8(3) 4_565 2_645 ?
N1 OH5 K2 155.6(3) 3_666 2_645 ?
N1 OH5 K2 75.7(2) 4_565 2_645 ?
O9 OH5 K2 65.7(2) 4_565 2_645 ?
N2 OH5 K2 120.7(3) 2_655 2_645 ?
C1 OH5 K2 59.3(2) 4_565 2_645 ?
OWB OH5 K2 100.3(7) 3_666 2_645 ?
O6 OH5 K2 122.0(3) 2_655 2_645 ?
OWA OH5 K2 98.1(4) 3_666 2_645 ?
P2 OH5 OWA 67.8(6) . 4_465 ?
O7 OH5 OWA 75.8(7) . 4_465 ?
O6 OH5 OWA 99.6(5) . 4_465 ?
O8 OH5 OWA 38.8(4) 1_545 4_465 ?
O10 OH5 OWA 59.2(7) 4_565 4_465 ?
N1 OH5 OWA 133.7(7) 3_666 4_465 ?
N1 OH5 OWA 130.4(5) 4_565 4_465 ?
O9 OH5 OWA 100.0(7) 4_565 4_465 ?
N2 OH5 OWA 96.3(4) 2_655 4_465 ?
C1 OH5 OWA 79.6(7) 4_565 4_465 ?
OWB OH5 OWA 47.4(8) 3_666 4_465 ?
O6 OH5 OWA 170.4(7) 2_655 4_465 ?
OWA OH5 OWA 48.64(15) 3_666 4_465 ?
K2 OH5 OWA 54.7(5) 2_645 4_465 ?
P2 OH5 OH1 159.3(4) . 2_655 ?
O7 OH5 OH1 137.9(3) . 2_655 ?
O6 OH5 OH1 124.5(3) . 2_655 ?
O8 OH5 OH1 160.2(3) 1_545 2_655 ?
O10 OH5 OH1 78.4(2) 4_565 2_655 ?
N1 OH5 OH1 75.3(2) 3_666 2_655 ?
N1 OH5 OH1 68.9(2) 4_565 2_655 ?
O9 OH5 OH1 51.18(18) 4_565 2_655 ?
N2 OH5 OH1 44.12(18) 2_655 2_655 ?
C1 OH5 OH1 62.6(2) 4_565 2_655 ?
OWB OH5 OH1 104.0(10) 3_666 2_655 ?
O6 OH5 OH1 38.34(17) 2_655 2_655 ?
OWA OH5 OH1 96.8(6) 3_666 2_655 ?
K2 OH5 OH1 116.8(2) 2_645 2_655 ?
OWA OH5 OH1 132.9(5) 4_465 2_655 ?
P2 OH5 OH1 51.7(3) . . ?
O7 OH5 OH1 48.1(2) . . ?
O6 OH5 OH1 34.8(2) . . ?
O8 OH5 OH1 86.1(3) 1_545 . ?
O10 OH5 OH1 164.6(4) 4_565 . ?
N1 OH5 OH1 45.49(18) 3_666 . ?
N1 OH5 OH1 74.8(2) 4_565 . ?
O9 OH5 OH1 130.2(3) 4_565 . ?
N2 OH5 OH1 128.5(3) 2_655 . ?
C1 OH5 OH1 151.4(3) 4_565 . ?
OWB OH5 OH1 117.0(13) 3_666 . ?
O6 OH5 OH1 71.5(2) 2_655 . ?
OWA OH5 OH1 126.3(7) 3_666 . ?
K2 OH5 OH1 110.5(2) 2_645 . ?
OWA OH5 OH1 118.0(6) 4_465 . ?
OH1 OH5 OH1 108.3(2) 2_655 . ?
P2 OH5 OWB 73.3(8) . 4_465 ?
O7 OH5 OWB 83.2(9) . 4_465 ?
O6 OH5 OWB 103.1(6) . 4_465 ?
O8 OH5 OWB 42.0(6) 1_545 4_465 ?
O10 OH5 OWB 52.0(8) 4_565 4_465 ?
N1 OH5 OWB 140.4(8) 3_666 4_465 ?
N1 OH5 OWB 126.1(7) 4_565 4_465 ?
O9 OH5 OWB 92.6(9) 4_565 4_465 ?
N2 OH5 OWB 93.6(5) 2_655 4_465 ?
C1 OH5 OWB 72.2(9) 4_565 4_465 ?
OWB OH5 OWB 50.0(5) 3_666 4_465 ?
O6 OH5 OWB 163.2(9) 2_655 4_465 ?
OWA OH5 OWB 49.6(7) 3_666 4_465 ?
K2 OH5 OWB 50.6(6) 2_645 4_465 ?
OWA OH5 OWB 7.4(5) 4_465 4_465 ?
OH1 OH5 OWB 127.2(7) 2_655 4_465 ?
OH1 OH5 OWB 124.3(8) . 4_465 ?
P2 OH5 O8 115.8(4) . . ?
O7 OH5 O8 80.1(3) . . ?
O6 OH5 O8 129.3(3) . . ?
O8 OH5 O8 126.7(4) 1_545 . ?
O10 OH5 O8 99.9(3) 4_565 . ?
N1 OH5 O8 53.6(2) 3_666 . ?
N1 OH5 O8 128.5(3) 4_565 . ?
O9 OH5 O8 109.7(2) 4_565 . ?
N2 OH5 O8 38.66(19) 2_655 . ?
C1 OH5 O8 104.2(3) 4_565 . ?
OWB OH5 O8 51.9(6) 3_666 . ?
O6 OH5 O8 80.8(2) 2_655 . ?
OWA OH5 O8 52.2(4) 3_666 . ?
K2 OH5 O8 149.4(3) 2_645 . ?
OWA OH5 O8 99.3(4) 4_465 . ?
OH1 OH5 O8 66.82(18) 2_655 . ?
OH1 OH5 O8 95.4(2) . . ?
OWB OH5 O8 101.5(5) 4_465 . ?
P2 OH5 O2 60.1(3) . 3_666 ?
O7 OH5 O2 24.2(2) . 3_666 ?
O6 OH5 O2 79.9(3) . 3_666 ?
O8 OH5 O2 82.6(3) 1_545 3_666 ?
O10 OH5 O2 133.4(3) 4_565 3_666 ?
N1 OH5 O2 50.18(17) 3_666 3_666 ?
N1 OH5 O2 130.9(2) 4_565 3_666 ?
O9 OH5 O2 165.7(3) 4_565 3_666 ?
N2 OH5 O2 93.6(2) 2_655 3_666 ?
C1 OH5 O2 151.7(3) 4_565 3_666 ?
OWB OH5 O2 60.5(12) 3_666 3_666 ?
O6 OH5 O2 103.7(2) 2_655 3_666 ?
OWA OH5 O2 69.5(7) 3_666 3_666 ?
K2 OH5 O2 126.3(2) 2_645 3_666 ?
OWA OH5 O2 83.9(6) 4_465 3_666 ?
OH1 OH5 O2 116.5(2) 2_655 3_666 ?
OH1 OH5 O2 56.83(15) . 3_666 ?
OWB OH5 O2 91.0(8) 4_465 3_666 ?
O8 OH5 O2 56.01(16) . 3_666 ?
P2 O6 O7 35.2(2) . . ?
P2 O6 OH5 37.5(3) . . ?
O7 O6 OH5 59.4(3) . . ?
P2 O6 O8 33.6(3) . 1_545 ?
O7 O6 O8 61.2(3) . 1_545 ?
OH5 O6 O8 59.7(3) . 1_545 ?
P2 O6 OH1 111.5(4) . . ?
O7 O6 OH1 77.3(3) . . ?
OH5 O6 OH1 112.3(4) . . ?
O8 O6 OH1 135.9(4) 1_545 . ?
P2 O6 N1 119.6(5) . 3_656 ?
O7 O6 N1 125.3(4) . 3_656 ?
OH5 O6 N1 140.8(4) . 3_656 ?
O8 O6 N1 87.5(3) 1_545 3_656 ?
OH1 O6 N1 106.3(3) . 3_656 ?
P2 O6 N1 105.4(4) . 4_565 ?
O7 O6 N1 126.4(4) . 4_565 ?
OH5 O6 N1 69.9(3) . 4_565 ?
O8 O6 N1 107.4(3) 1_545 4_565 ?
OH1 O6 N1 109.1(3) . 4_565 ?
N1 O6 N1 104.4(3) 3_656 4_565 ?
P2 O6 OH5 159.9(4) . 2_645 ?
O7 O6 OH5 163.6(4) . 2_645 ?
OH5 O6 OH5 128.0(3) . 2_645 ?
O8 O6 OH5 134.8(4) 1_545 2_645 ?
OH1 O6 OH5 86.3(3) . 2_645 ?
N1 O6 OH5 60.4(2) 3_656 2_645 ?
N1 O6 OH5 58.1(2) 4_565 2_645 ?
P2 O6 O4 65.5(3) . 3_656 ?
O7 O6 O4 49.1(2) . 3_656 ?
OH5 O6 O4 102.1(3) . 3_656 ?
O8 O6 O4 62.1(2) 1_545 3_656 ?
OH1 O6 O4 80.0(2) . 3_656 ?
N1 O6 O4 77.1(2) 3_656 3_656 ?
N1 O6 O4 169.5(3) 4_565 3_656 ?
OH5 O6 O4 129.4(3) 2_645 3_656 ?
P2 O6 N1 72.7(3) . 3_666 ?
O7 O6 N1 55.2(2) . 3_666 ?
OH5 O6 N1 58.1(3) . 3_666 ?
O8 O6 N1 106.2(3) 1_545 3_666 ?
OH1 O6 N1 54.5(2) . 3_666 ?
N1 O6 N1 160.8(3) 3_656 3_666 ?
N1 O6 N1 84.6(3) 4_565 3_666 ?
OH5 O6 N1 113.7(3) 2_645 3_666 ?
O4 O6 N1 97.2(2) 3_656 3_666 ?
P2 O6 O3 105.3(3) . 3_656 ?
O7 O6 O3 84.7(2) . 3_656 ?
OH5 O6 O3 141.9(3) . 3_656 ?
O8 O6 O3 93.5(3) 1_545 3_656 ?
OH1 O6 O3 66.8(2) . 3_656 ?
N1 O6 O3 51.5(2) 3_656 3_656 ?
N1 O6 O3 148.0(3) 4_565 3_656 ?
OH5 O6 O3 90.0(2) 2_645 3_656 ?
O4 O6 O3 39.91(14) 3_656 3_656 ?
N1 O6 O3 113.0(2) 3_666 3_656 ?
P2 O6 P1 102.4(3) . . ?
O7 O6 P1 67.2(2) . . ?
OH5 O6 P1 115.8(3) . . ?
O8 O6 P1 119.6(3) 1_545 . ?
OH1 O6 P1 19.06(14) . . ?
N1 O6 P1 98.4(3) 3_656 . ?
N1 O6 P1 128.2(3) 4_565 . ?
OH5 O6 P1 97.3(2) 2_645 . ?
O4 O6 P1 61.08(16) 3_656 . ?
N1 O6 P1 63.34(16) 3_666 . ?
O3 O6 P1 51.59(15) 3_656 . ?
P2 O6 Fe 54.6(3) . . ?
O7 O6 Fe 24.24(16) . . ?
OH5 O6 Fe 83.6(3) . . ?
O8 O6 Fe 69.9(2) 1_545 . ?
OH1 O6 Fe 66.1(2) . . ?
N1 O6 Fe 106.1(3) 3_656 . ?
N1 O6 Fe 149.2(3) 4_565 . ?
OH5 O6 Fe 145.3(3) 2_645 . ?
O4 O6 Fe 29.63(13) 3_656 . ?
N1 O6 Fe 67.71(16) 3_666 . ?
O3 O6 Fe 60.70(15) 3_656 . ?
P1 O6 Fe 50.68(11) . . ?
P2 O6 O3 81.6(3) . . ?
O7 O6 O3 47.48(19) . . ?
OH5 O6 O3 103.8(3) . . ?
O8 O6 O3 96.9(3) 1_545 . ?
OH1 O6 O3 39.99(18) . . ?
N1 O6 O3 100.8(3) 3_656 . ?
N1 O6 O3 145.4(3) 4_565 . ?
OH5 O6 O3 118.5(3) 2_645 . ?
O4 O6 O3 41.72(15) 3_656 . ?
N1 O6 O3 64.86(18) 3_666 . ?
O3 O6 O3 49.3(2) 3_656 . ?
P1 O6 O3 22.84(9) . . ?
Fe O6 O3 28.04(10) . . ?
P2 O6 K2 66.9(3) . 2_645 ?
O7 O6 K2 100.5(3) . 2_645 ?
OH5 O6 K2 68.9(3) . 2_645 ?
O8 O6 K2 41.0(2) 1_545 2_645 ?
OH1 O6 K2 176.0(3) . 2_645 ?
N1 O6 K2 72.2(2) 3_656 2_645 ?
N1 O6 K2 74.9(2) 4_565 2_645 ?
OH5 O6 K2 95.9(2) 2_645 2_645 ?
O4 O6 K2 96.0(2) 3_656 2_645 ?
N1 O6 K2 126.9(3) 3_666 2_645 ?
O3 O6 K2 109.8(3) 3_656 2_645 ?
P1 O6 K2 156.9(2) . 2_645 ?
Fe O6 K2 110.6(2) . 2_645 ?
O3 O6 K2 136.2(2) . 2_645 ?
P2 O6 O6 91.1(3) . 2_655 ?
O7 O6 O6 93.5(2) . 2_655 ?
OH5 O6 O6 55.9(2) . 2_655 ?
O8 O6 O6 114.7(4) 1_545 2_655 ?
OH1 O6 O6 80.4(3) . 2_655 ?
N1 O6 O6 141.2(3) 3_656 2_655 ?
N1 O6 O6 40.3(2) 4_565 2_655 ?
OH5 O6 O6 82.5(3) 2_645 2_655 ?
O4 O6 O6 140.9(2) 3_656 2_655 ?
N1 O6 O6 44.34(10) 3_666 2_655 ?
O3 O6 O6 146.8(3) 3_656 2_655 ?
P1 O6 O6 97.2(2) . 2_655 ?
Fe O6 O6 111.25(17) . 2_655 ?
O3 O6 O6 107.1(2) . 2_655 ?
K2 O6 O6 103.2(3) 2_645 2_655 ?
P2 O6 O6 127.0(5) . 2_645 ?
O7 O6 O6 159.4(4) . 2_645 ?
OH5 O6 O6 113.9(4) . 2_645 ?
O8 O6 O6 98.3(3) 1_545 2_645 ?
OH1 O6 O6 121.6(4) . 2_645 ?
N1 O6 O6 45.71(13) 3_656 2_645 ?
N1 O6 O6 58.8(3) 4_565 2_645 ?
OH5 O6 O6 36.5(2) 2_645 2_645 ?
O4 O6 O6 121.5(2) 3_656 2_645 ?
N1 O6 O6 140.8(3) 3_666 2_645 ?
O3 O6 O6 95.1(2) 3_656 2_645 ?
P1 O6 O6 127.8(3) . 2_645 ?
Fe O6 O6 151.1(2) . 2_645 ?
O3 O6 O6 142.1(3) . 2_645 ?
K2 O6 O6 60.2(2) 2_645 2_645 ?
O6 O6 O6 97.7(3) 2_655 2_645 ?
P2 O6 K2 141.5(5) . . ?
O7 O6 K2 116.0(3) . . ?
OH5 O6 K2 114.6(3) . . ?
O8 O6 K2 174.3(4) 1_545 . ?
OH1 O6 K2 43.9(2) . . ?
N1 O6 K2 98.0(3) 3_656 . ?
N1 O6 K2 69.8(2) 4_565 . ?
OH5 O6 K2 48.4(2) 2_645 . ?
O4 O6 K2 120.6(2) 3_656 . ?
N1 O6 K2 68.8(2) 3_666 . ?
O3 O6 K2 91.2(2) 3_656 . ?
P1 O6 K2 61.29(16) . . ?
Fe O6 K2 109.8(2) . . ?
O3 O6 K2 83.7(2) . . ?
K2 O6 K2 139.6(2) 2_645 . ?
O6 O6 K2 59.9(2) 2_655 . ?
O6 O6 K2 84.6(3) 2_645 . ?
P2 O6 O4 115.9(3) . . ?
O7 O6 O4 82.2(2) . . ?
OH5 O6 O4 135.1(3) . . ?
O8 O6 O4 122.8(3) 1_545 . ?
OH1 O6 O4 29.95(19) . . ?
N1 O6 O4 79.4(2) 3_656 . ?
N1 O6 O4 129.8(3) 4_565 . ?
OH5 O6 O4 84.2(2) 2_645 . ?
O4 O6 O4 60.69(19) 3_656 . ?
N1 O6 O4 81.85(19) 3_666 . ?
O3 O6 O4 37.20(14) 3_656 . ?
P1 O6 O4 19.48(10) . . ?
Fe O6 O4 61.34(14) . . ?
O3 O6 O4 34.69(13) . . ?
K2 O6 O4 146.9(3) 2_645 . ?
O6 O6 O4 109.6(3) 2_655 . ?
O6 O6 O4 109.9(3) 2_645 . ?
K2 O6 O4 60.24(17) . . ?
P2 O7 Fe 142.0(5) . . ?
P2 O7 OH5 38.0(3) . . ?
Fe O7 OH5 174.4(4) . . ?
P2 O7 O6 36.4(3) . . ?
Fe O7 O6 123.0(4) . . ?
OH5 O7 O6 60.6(3) . . ?
P2 O7 O8 32.4(3) . 1_545 ?
Fe O7 O8 117.3(4) . 1_545 ?
OH5 O7 O8 59.9(3) . 1_545 ?
O6 O7 O8 60.7(3) . 1_545 ?
P2 O7 O2 171.4(4) . 3_666 ?
Fe O7 O2 46.4(2) . 3_666 ?
OH5 O7 O2 133.5(4) . 3_666 ?
O6 O7 O2 147.1(3) . 3_666 ?
O8 O7 O2 150.1(3) 1_545 3_666 ?
P2 O7 O11 120.9(4) . . ?
Fe O7 O11 48.15(19) . . ?
OH5 O7 O11 126.3(3) . . ?
O6 O7 O11 141.2(4) . . ?
O8 O7 O11 88.9(3) 1_545 . ?
O2 O7 O11 61.6(2) 3_666 . ?
P2 O7 O4 98.0(4) . 3_656 ?
Fe O7 O4 44.0(2) . 3_656 ?
OH5 O7 O4 135.3(4) . 3_656 ?
O6 O7 O4 88.2(3) . 3_656 ?
O8 O7 O4 77.5(3) 1_545 3_656 ?
O2 O7 O4 90.3(2) 3_666 3_656 ?
O11 O7 O4 60.3(2) . 3_656 ?
P2 O7 O3 127.8(4) . . ?
Fe O7 O3 39.75(17) . . ?
OH5 O7 O3 145.8(3) . . ?
O6 O7 O3 93.4(3) . . ?
O8 O7 O3 128.9(4) 1_545 . ?
O2 O7 O3 59.1(2) 3_666 . ?
O11 O7 O3 87.9(2) . . ?
O4 O7 O3 57.1(2) 3_656 . ?
P2 O7 N1 96.2(3) . 3_666 ?
Fe O7 N1 114.5(3) . 3_666 ?
OH5 O7 N1 69.4(3) . 3_666 ?
O6 O7 N1 82.8(3) . 3_666 ?
O8 O7 N1 127.1(3) 1_545 3_666 ?
O2 O7 N1 78.4(3) 3_666 3_666 ?
O11 O7 N1 135.9(3) . 3_666 ?
O4 O7 N1 142.2(3) 3_656 3_666 ?
O3 O7 N1 86.7(2) . 3_666 ?
P2 O7 OH1 88.9(3) . . ?
Fe O7 OH1 88.9(2) . . ?
OH5 O7 OH1 96.7(3) . . ?
O6 O7 OH1 53.3(2) . . ?
O8 O7 OH1 112.4(3) 1_545 . ?
O2 O7 OH1 93.8(2) 3_666 . ?
O11 O7 OH1 136.8(3) . . ?
O4 O7 OH1 87.1(2) 3_656 . ?
O3 O7 OH1 49.26(17) . . ?
N1 O7 OH1 58.3(2) 3_666 . ?
P2 O7 OWB 87.4(7) . 3_666 ?
Fe O7 OWB 109.9(8) . 3_666 ?
OH5 O7 OWB 65.1(8) . 3_666 ?
O6 O7 OWB 122.3(7) . 3_666 ?
O8 O7 OWB 76.5(6) 1_545 3_666 ?
O2 O7 OWB 86.5(7) 3_666 3_666 ?
O11 O7 OWB 65.6(7) . 3_666 ?
O4 O7 OWB 119.6(7) 3_656 3_666 ?
O3 O7 OWB 144.3(7) . 3_666 ?
N1 O7 OWB 95.9(6) 3_666 3_666 ?
OH1 O7 OWB 153.3(7) . 3_666 ?
P2 O7 P1 110.5(3) . . ?
Fe O7 P1 63.24(18) . . ?
OH5 O7 P1 122.3(3) . . ?
O6 O7 P1 74.2(2) . . ?
O8 O7 P1 125.0(3) 1_545 . ?
O2 O7 P1 74.32(19) 3_666 . ?
O11 O7 P1 111.4(2) . . ?
O4 O7 P1 70.97(18) 3_656 . ?
O3 O7 P1 23.52(12) . . ?
N1 O7 P1 71.25(17) 3_666 . ?
OH1 O7 P1 25.77(12) . . ?
OWB O7 P1 158.5(6) 3_666 . ?
P2 O7 K 128.0(3) . 3_666 ?
Fe O7 K 80.3(2) . 3_666 ?
OH5 O7 K 96.6(3) . 3_666 ?
O6 O7 K 156.1(3) . 3_666 ?
O8 O7 K 116.3(3) 1_545 3_666 ?
O2 O7 K 45.05(18) 3_666 3_666 ?
O11 O7 K 57.1(2) . 3_666 ?
O4 O7 K 114.9(2) 3_656 3_666 ?
O3 O7 K 104.1(2) . 3_666 ?
N1 O7 K 82.0(2) 3_666 3_666 ?
OH1 O7 K 129.6(2) . 3_666 ?
OWB O7 K 41.8(6) 3_666 3_666 ?
P1 O7 K 117.61(18) . 3_666 ?
P2 O7 P1 159.0(4) . 3_666 ?
Fe O7 P1 57.0(2) . 3_666 ?
OH5 O7 P1 124.3(3) . 3_666 ?
O6 O7 P1 134.1(3) . 3_666 ?
O8 O7 P1 165.2(3) 1_545 3_666 ?
O2 O7 P1 16.01(15) 3_666 3_666 ?
O11 O7 P1 77.5(2) . 3_666 ?
O4 O7 P1 100.3(2) 3_656 3_666 ?
O3 O7 P1 57.26(18) . 3_666 ?
N1 O7 P1 62.96(18) 3_666 3_666 ?
OH1 O7 P1 81.90(18) . 3_666 ?
OWB O7 P1 92.4(6) 3_666 3_666 ?
P1 O7 P1 66.64(12) . 3_666 ?
K O7 P1 51.01(11) 3_666 3_666 ?
P2 O7 OWA 84.3(4) . 3_666 ?
Fe O7 OWA 113.6(4) . 3_666 ?
OH5 O7 OWA 61.4(4) . 3_666 ?
O6 O7 OWA 118.8(4) . 3_666 ?
O8 O7 OWA 74.8(4) 1_545 3_666 ?
O2 O7 OWA 89.4(4) 3_666 3_666 ?
O11 O7 OWA 69.1(4) . 3_666 ?
O4 O7 OWA 121.9(4) 3_656 3_666 ?
O3 O7 OWA 147.7(4) . 3_666 ?
N1 O7 OWA 94.2(4) 3_666 3_666 ?
OH1 O7 OWA 150.8(4) . 3_666 ?
OWB O7 OWA 3.7(8) 3_666 3_666 ?
P1 O7 OWA 159.9(4) . 3_666 ?
K O7 OWA 44.5(3) 3_666 3_666 ?
P1 O7 OWA 94.6(4) 3_666 3_666 ?
P2 O7 O3 140.5(3) . 3_666 ?
Fe O7 O3 67.8(2) . 3_666 ?
OH5 O7 O3 115.6(3) . 3_666 ?
O6 O7 O3 112.2(3) . 3_666 ?
O8 O7 O3 172.6(3) 1_545 3_666 ?
O2 O7 O3 37.30(18) 3_666 3_666 ?
O11 O7 O3 98.5(2) . 3_666 ?
O4 O7 O3 105.2(2) 3_656 3_666 ?
O3 O7 O3 50.9(2) . 3_666 ?
N1 O7 O3 47.01(16) 3_666 3_666 ?
OH1 O7 O3 61.28(18) . 3_666 ?
OWB O7 O3 107.4(6) 3_666 3_666 ?
P1 O7 O3 51.20(13) . 3_666 ?
K O7 O3 69.13(15) 3_666 3_666 ?
P1 O7 O3 22.04(9) 3_666 3_666 ?
OWA O7 O3 108.7(4) 3_666 3_666 ?
P2 O7 K 73.5(3) . 3_656 ?
Fe O7 K 74.5(2) . 3_656 ?
OH5 O7 K 102.0(3) . 3_656 ?
O6 O7 K 87.8(3) . 3_656 ?
O8 O7 K 43.1(2) 1_545 3_656 ?
O2 O7 K 112.0(2) 3_666 3_656 ?
O11 O7 K 53.77(19) . 3_656 ?
O4 O7 K 41.32(17) 3_656 3_656 ?
O3 O7 K 98.4(2) . 3_656 ?
N1 O7 K 169.6(2) 3_666 3_656 ?
OH1 O7 K 118.9(2) . 3_656 ?
OWB O7 K 85.3(6) 3_666 3_656 ?
P1 O7 K 110.53(17) . 3_656 ?
K O7 K 105.30(16) 3_666 3_656 ?
P1 O7 K 127.38(16) 3_666 3_656 ?
OWA O7 K 86.3(3) 3_666 3_656 ?
O3 O7 K 142.27(18) 3_666 3_656 ?
P2 O7 P1 91.5(3) . 3_656 ?
Fe O7 P1 51.31(19) . 3_656 ?
OH5 O7 P1 129.5(3) . 3_656 ?
O6 O7 P1 76.5(3) . 3_656 ?
O8 O7 P1 77.0(3) 1_545 3_656 ?
O2 O7 P1 97.0(2) 3_666 3_656 ?
O11 O7 P1 73.4(2) . 3_656 ?
O4 O7 P1 13.10(14) 3_656 3_656 ?
O3 O7 P1 53.40(18) . 3_656 ?
N1 O7 P1 132.9(2) 3_666 3_656 ?
OH1 O7 P1 75.56(17) . 3_656 ?
OWB O7 P1 131.0(6) 3_666 3_656 ?
P1 O7 P1 62.54(12) . 3_656 ?
K O7 P1 127.09(16) 3_666 3_656 ?
P1 O7 P1 104.22(15) 3_666 3_656 ?
OWA O7 P1 132.9(4) 3_666 3_656 ?
O3 O7 P1 104.05(17) 3_666 3_656 ?
K O7 P1 48.01(10) 3_656 3_656 ?
P2 O8 OH5 36.7(3) 1_565 1_565 ?
P2 O8 O6 34.3(3) 1_565 1_565 ?
OH5 O8 O6 59.2(3) 1_565 1_565 ?
P2 O8 O7 32.0(2) 1_565 1_565 ?
OH5 O8 O7 58.2(3) 1_565 1_565 ?
O6 O8 O7 58.1(3) 1_565 1_565 ?
P2 O8 OWA 128.1(8) 1_565 4_475 ?
OH5 O8 OWA 104.5(6) 1_565 4_475 ?
O6 O8 OWA 162.1(7) 1_565 4_475 ?
O7 O8 OWA 108.3(9) 1_565 4_475 ?
P2 O8 N2 122.6(4) 1_565 2_655 ?
OH5 O8 N2 98.1(3) 1_565 2_655 ?
O6 O8 N2 102.6(4) 1_565 2_655 ?
O7 O8 N2 154.2(4) 1_565 2_655 ?
OWA O8 N2 86.2(10) 4_475 2_655 ?
P2 O8 K 127.2(4) 1_565 3_666 ?
OH5 O8 K 153.7(4) 1_565 3_666 ?
O6 O8 K 122.0(3) 1_565 3_666 ?
O7 O8 K 98.7(3) 1_565 3_666 ?
OWA O8 K 68.8(6) 4_475 3_666 ?
N2 O8 K 106.5(3) 2_655 3_666 ?
P2 O8 OWB 133.4(9) 1_565 4_475 ?
OH5 O8 OWB 104.9(7) 1_565 4_475 ?
O6 O8 OWB 163.9(7) 1_565 4_475 ?
O7 O8 OWB 117.2(11) 1_565 4_475 ?
OWA O8 OWB 10.0(8) 4_475 4_475 ?
N2 O8 OWB 76.2(11) 2_655 4_475 ?
K O8 OWB 73.0(7) 3_666 4_475 ?
P2 O8 O4 76.5(3) 1_565 3_666 ?
OH5 O8 O4 111.0(3) 1_565 3_666 ?
O6 O8 O4 75.5(3) 1_565 3_666 ?
O7 O8 O4 54.1(2) 1_565 3_666 ?
OWA O8 O4 106.8(8) 4_475 3_666 ?
N2 O8 O4 143.2(4) 2_655 3_666 ?
K O8 O4 51.52(18) 3_666 3_666 ?
OWB O8 O4 115.2(10) 4_475 3_666 ?
P2 O8 O10 86.0(4) 1_565 4_575 ?
OH5 O8 O10 49.3(2) 1_565 4_575 ?
O6 O8 O10 100.4(3) 1_565 4_575 ?
O7 O8 O10 101.8(3) 1_565 4_575 ?
OWA O8 O10 69.5(6) 4_475 4_575 ?
N2 O8 O10 62.6(3) 2_655 4_575 ?
K O8 O10 137.5(3) 3_666 4_575 ?
OWB O8 O10 64.5(8) 4_475 4_575 ?
O4 O8 O10 154.2(3) 3_666 4_575 ?
P2 O8 OWB 164.4(13) 1_565 3_666 ?
OH5 O8 OWB 155.4(12) 1_565 3_666 ?
O6 O8 OWB 131.9(10) 1_565 3_666 ?
O7 O8 OWB 145.4(10) 1_565 3_666 ?
OWA O8 OWB 66.0(9) 4_475 3_666 ?
N2 O8 OWB 59.8(8) 2_655 3_666 ?
K O8 OWB 46.8(9) 3_666 3_666 ?
OWB O8 OWB 61.7(8) 4_475 3_666 ?
O4 O8 OWB 93.5(11) 3_666 3_666 ?
O10 O8 OWB 107.1(13) 4_575 3_666 ?
P2 O8 OWA 173.5(8) 1_565 3_666 ?
OH5 O8 OWA 145.9(8) 1_565 3_666 ?
O6 O8 OWA 139.2(7) 1_565 3_666 ?
O7 O8 OWA 151.1(5) 1_565 3_666 ?
OWA O8 OWA 58.4(3) 4_475 3_666 ?
N2 O8 OWA 54.6(5) 2_655 3_666 ?
K O8 OWA 53.4(6) 3_666 3_666 ?
OWB O8 OWA 52.9(8) 4_475 3_666 ?
O4 O8 OWA 102.6(7) 3_666 3_666 ?
O10 O8 OWA 96.8(8) 4_575 3_666 ?
OWB O8 OWA 10.6(7) 3_666 3_666 ?
P2 O8 N1 81.5(4) 1_565 3_666 ?
OH5 O8 N1 104.4(3) 1_565 3_666 ?
O6 O8 N1 48.2(3) 1_565 3_666 ?
O7 O8 N1 94.6(3) 1_565 3_666 ?
OWA O8 N1 149.7(6) 4_475 3_666 ?
N2 O8 N1 80.9(3) 2_655 3_666 ?
K O8 N1 88.7(2) 3_666 3_666 ?
OWB O8 N1 144.9(9) 4_475 3_666 ?
O4 O8 N1 70.6(2) 3_666 3_666 ?
O10 O8 N1 125.8(3) 4_575 3_666 ?
OWB O8 N1 83.8(10) 3_666 3_666 ?
OWA O8 N1 92.1(7) 3_666 3_666 ?
P2 O8 O11 78.9(3) 1_565 1_565 ?
OH5 O8 O11 94.3(3) 1_565 1_565 ?
O6 O8 O11 101.7(3) 1_565 1_565 ?
O7 O8 O11 47.1(2) 1_565 1_565 ?
OWA O8 O11 70.5(10) 4_475 1_565 ?
N2 O8 O11 155.7(3) 2_655 1_565 ?
K O8 O11 59.4(2) 3_666 1_565 ?
OWB O8 O11 80.5(11) 4_475 1_565 ?
O4 O8 O11 45.72(17) 3_666 1_565 ?
O10 O8 O11 112.7(3) 4_575 1_565 ?
OWB O8 O11 102.9(6) 3_666 1_565 ?
OWA O8 O11 105.2(4) 3_666 1_565 ?
N1 O8 O11 116.0(2) 3_666 1_565 ?
P2 O8 OWB 75.0(8) 1_565 3_676 ?
OH5 O8 OWB 58.9(5) 1_565 3_676 ?
O6 O8 OWB 109.1(7) 1_565 3_676 ?
O7 O8 OWB 62.1(10) 1_565 3_676 ?
OWA O8 OWB 53.1(12) 4_475 3_676 ?
N2 O8 OWB 116.8(11) 2_655 3_676 ?
K O8 OWB 100.8(7) 3_666 3_676 ?
OWB O8 OWB 59.1(13) 4_475 3_676 ?
O4 O8 OWB 97.8(10) 3_666 3_676 ?
O10 O8 OWB 58.9(9) 4_575 3_676 ?
OWB O8 OWB 118.8(14) 3_666 3_676 ?
OWA O8 OWB 111.5(12) 3_666 3_676 ?
N1 O8 OWB 155.8(9) 3_666 3_676 ?
O11 O8 OWB 53.9(9) 1_565 3_676 ?
P2 O8 Al 55.6(3) 1_565 1_565 ?
OH5 O8 Al 84.1(3) 1_565 1_565 ?
O6 O8 Al 71.3(2) 1_565 1_565 ?
O7 O8 Al 26.03(16) 1_565 1_565 ?
OWA O8 Al 101.5(10) 4_475 1_565 ?
N2 O8 Al 171.2(4) 2_655 1_565 ?
K O8 Al 72.91(18) 3_666 1_565 ?
OWB O8 Al 111.5(11) 4_475 1_565 ?
O4 O8 Al 30.37(14) 3_666 1_565 ?
O10 O8 Al 123.9(3) 4_575 1_565 ?
OWB O8 Al 119.4(10) 3_666 1_565 ?
OWA O8 Al 126.1(6) 3_666 1_565 ?
N1 O8 Al 90.34(19) 3_666 1_565 ?
O11 O8 Al 31.10(11) 1_565 1_565 ?
OWB O8 Al 71.6(10) 3_676 1_565 ?
P2 O8 OWA 79.1(5) 1_565 3_676 ?
OH5 O8 OWA 58.7(4) 1_565 3_676 ?
O6 O8 OWA 112.6(5) 1_565 3_676 ?
O7 O8 OWA 69.0(6) 1_565 3_676 ?
OWA O8 OWA 49.5(7) 4_475 3_676 ?
N2 O8 OWA 109.3(6) 2_655 3_676 ?
K O8 OWA 103.4(4) 3_666 3_676 ?
OWB O8 OWA 54.3(11) 4_475 3_676 ?
O4 O8 OWA 105.0(6) 3_666 3_676 ?
O10 O8 OWA 52.3(5) 4_575 3_676 ?
OWB O8 OWA 115.4(12) 3_666 3_676 ?
OWA O8 OWA 107.2(10) 3_666 3_676 ?
N1 O8 OWA 160.7(5) 3_666 3_676 ?
O11 O8 OWA 60.5(5) 1_565 3_676 ?
OWB O8 OWA 7.5(7) 3_676 3_676 ?
Al O8 OWA 79.1(6) 1_565 3_676 ?
P2 O8 O2 102.8(4) 1_565 3_666 ?
OH5 O8 O2 139.5(3) 1_565 3_666 ?
O6 O8 O2 85.3(3) 1_565 3_666 ?
O7 O8 O2 87.7(3) 1_565 3_666 ?
OWA O8 O2 106.8(6) 4_475 3_666 ?
N2 O8 O2 108.8(3) 2_655 3_666 ?
K O8 O2 38.02(14) 3_666 3_666 ?
OWB O8 O2 110.4(7) 4_475 3_666 ?
O4 O8 O2 34.74(16) 3_666 3_666 ?
O10 O8 O2 170.4(3) 4_575 3_666 ?
OWB O8 O2 63.6(12) 3_666 3_666 ?
OWA O8 O2 74.0(8) 3_666 3_666 ?
N1 O8 O2 53.23(17) 3_666 3_666 ?
O11 O8 O2 73.16(19) 1_565 3_666 ?
OWB O8 O2 126.6(9) 3_676 3_666 ?
Al O8 O2 65.11(16) 1_565 3_666 ?
OWA O8 O2 132.4(5) 3_676 3_666 ?
P2 O8 OH5 122.3(5) 1_565 . ?
OH5 O8 OH5 126.7(4) 1_565 . ?
O6 O8 OH5 88.2(3) 1_565 . ?
O7 O8 OH5 138.7(3) 1_565 . ?
OWA O8 OH5 108.8(8) 4_475 . ?
N2 O8 OH5 45.6(2) 2_655 . ?
K O8 OH5 78.5(2) 3_666 . ?
OWB O8 OH5 101.5(9) 4_475 . ?
O4 O8 OH5 97.8(2) 3_666 . ?
O10 O8 OH5 107.6(2) 4_575 . ?
OWB O8 OH5 46.3(7) 3_666 . ?
OWA O8 OH5 51.3(5) 3_666 . ?
N1 O8 OH5 44.53(17) 3_666 . ?
O11 O8 OH5 135.7(2) 1_565 . ?
OWB O8 OH5 159.1(10) 3_676 . ?
Al O8 OH5 126.7(2) 1_565 . ?
OWA O8 OH5 152.2(6) 3_676 . ?
O2 O8 OH5 64.62(18) 3_666 . ?
P2 O8 K1 51.4(3) 1_565 4_575 ?
OH5 O8 K1 43.6(3) 1_565 4_575 ?
O6 O8 K1 39.8(2) 1_565 4_575 ?
O7 O8 K1 83.4(2) 1_565 4_575 ?
OWA O8 K1 133.9(7) 4_475 4_575 ?
N2 O8 K1 71.5(2) 2_655 4_575 ?
K O8 K1 155.4(3) 3_666 4_575 ?
OWB O8 K1 127.8(9) 4_475 4_575 ?
O4 O8 K1 115.3(2) 3_666 4_575 ?
O10 O8 K1 64.48(18) 4_575 4_575 ?
OWB O8 K1 126.3(6) 3_666 4_575 ?
OWA O8 K1 124.8(4) 3_666 4_575 ?
N1 O8 K1 66.76(17) 3_666 4_575 ?
O11 O8 K1 130.0(2) 1_565 4_575 ?
OWB O8 K1 101.8(6) 3_676 4_575 ?
Al O8 K1 105.29(19) 1_565 4_575 ?
OWA O8 K1 100.2(4) 3_676 4_575 ?
O2 O8 K1 118.2(2) 3_666 4_575 ?
OH5 O8 K1 83.8(2) . 4_575 ?
C1 O9 Fe 114.9(5) . . ?
C1 O9 O2 104.8(6) . 3_666 ?
Fe O9 O2 45.6(2) . 3_666 ?
C1 O9 O3 158.5(5) . . ?
Fe O9 O3 43.64(17) . . ?
O2 O9 O3 60.9(2) 3_666 . ?
C1 O9 O4 107.8(6) . 3_656 ?
Fe O9 O4 44.3(2) . 3_656 ?
O2 O9 O4 89.9(2) 3_666 3_656 ?
O3 O9 O4 59.2(2) . 3_656 ?
C1 O9 K1 136.7(6) . . ?
Fe O9 K1 105.0(2) . . ?
O2 O9 K1 90.9(3) 3_666 . ?
O3 O9 K1 63.0(2) . . ?
O4 O9 K1 112.3(3) 3_656 . ?
C1 O9 OH5 81.4(5) . 4_566 ?
Fe O9 OH5 162.9(3) . 4_566 ?
O2 O9 OH5 138.4(3) 3_666 4_566 ?
O3 O9 OH5 120.1(3) . 4_566 ?
O4 O9 OH5 128.0(3) 3_656 4_566 ?
K1 O9 OH5 61.5(2) . 4_566 ?
C1 O9 OH1 111.6(6) . 3_656 ?
Fe O9 OH1 88.5(3) . 3_656 ?
O2 O9 OH1 130.9(3) 3_666 3_656 ?
O3 O9 OH1 73.9(2) . 3_656 ?
O4 O9 OH1 48.4(2) 3_656 3_656 ?
K1 O9 OH1 84.7(2) . 3_656 ?
OH5 O9 OH1 80.1(2) 4_566 3_656 ?
C1 O9 OH1 107.8(6) . 3_666 ?
Fe O9 OH1 88.0(3) . 3_666 ?
O2 O9 OH1 46.8(2) 3_666 3_666 ?
O3 O9 OH1 74.9(2) . 3_666 ?
O4 O9 OH1 129.4(3) 3_656 3_666 ?
K1 O9 OH1 55.95(19) . 3_666 ?
OH5 O9 OH1 91.9(2) 4_566 3_666 ?
OH1 O9 OH1 137.9(3) 3_656 3_666 ?
C1 O10 OH5 109.2(6) . 4_566 ?
C1 O10 K 122.5(6) . 1_455 ?
OH5 O10 K 126.5(3) 4_566 1_455 ?
C1 O10 K2 93.2(6) . 3_656 ?
OH5 O10 K2 65.7(3) 4_566 3_656 ?
K O10 K2 97.0(3) 1_455 3_656 ?
C1 O10 K2 96.6(7) . 3_666 ?
OH5 O10 K2 84.6(3) 4_566 3_666 ?
K O10 K2 101.1(3) 1_455 3_666 ?
K2 O10 K2 150.3(3) 3_656 3_666 ?
C1 O10 OWA 145.4(9) . 2_646 ?
OH5 O10 OWA 71.2(8) 4_566 2_646 ?
K O10 OWA 58.9(7) 1_455 2_646 ?
K2 O10 OWA 54.4(4) 3_656 2_646 ?
K2 O10 OWA 117.6(7) 3_666 2_646 ?
C1 O10 O8 131.8(6) . 4_576 ?
OH5 O10 O8 46.2(2) 4_566 4_576 ?
K O10 O8 99.5(2) 1_455 4_576 ?
K2 O10 O8 104.9(3) 3_656 4_576 ?
K2 O10 O8 49.1(2) 3_666 4_576 ?
OWA O10 O8 74.8(8) 2_646 4_576 ?
C1 O10 OWB 150.9(13) . 1_455 ?
OH5 O10 OWB 91.7(13) 4_566 1_455 ?
K O10 OWB 47.8(9) 1_455 1_455 ?
K2 O10 OWB 114.2(9) 3_656 1_455 ?
K2 O10 OWB 64.6(6) 3_666 1_455 ?
OWA O10 OWB 59.8(9) 2_646 1_455 ?
O8 O10 OWB 52.5(11) 4_576 1_455 ?
C1 O10 OWA 159.3(9) . 1_455 ?
OH5 O10 OWA 80.9(9) 4_566 1_455 ?
K O10 OWA 55.4(7) 1_455 1_455 ?
K2 O10 OWA 107.5(7) 3_656 1_455 ?
K2 O10 OWA 65.8(4) 3_666 1_455 ?
OWA O10 OWA 54.31(14) 2_646 1_455 ?
O8 O10 OWA 44.1(7) 4_576 1_455 ?
OWB O10 OWA 10.9(7) 1_455 1_455 ?
C1 O10 OWB 150.0(9) . 2_646 ?
OH5 O10 OWB 61.6(11) 4_566 2_646 ?
K O10 OWB 66.7(10) 1_455 2_646 ?
K2 O10 OWB 56.8(6) 3_656 2_646 ?
K2 O10 OWB 110.0(10) 3_666 2_646 ?
OWA O10 OWB 10.8(7) 2_646 2_646 ?
O8 O10 OWB 64.9(12) 4_576 2_646 ?
OWB O10 OWB 58.1(8) 1_455 2_646 ?
OWA O10 OWB 50.6(7) 1_455 2_646 ?
C2 O11 Fe 114.8(6) . . ?
C2 O11 O7 158.6(6) . . ?
Fe O11 O7 44.11(18) . . ?
C2 O11 O2 105.1(6) . 3_666 ?
Fe O11 O2 44.5(2) . 3_666 ?
O7 O11 O2 58.4(2) . 3_666 ?
C2 O11 O4 108.4(6) . 3_656 ?
Fe O11 O4 44.5(2) . 3_656 ?
O7 O11 O4 61.1(2) . 3_656 ?
O2 O11 O4 89.0(2) 3_666 3_656 ?
C2 O11 K 102.1(6) . 3_666 ?
Fe O11 K 94.5(2) . 3_666 ?
O7 O11 K 79.3(2) . 3_666 ?
O2 O11 K 52.76(18) 3_666 3_666 ?
O4 O11 K 136.4(3) 3_656 3_666 ?
C2 O11 K 103.3(6) . 3_656 ?
Fe O11 K 94.9(2) . 3_656 ?
O7 O11 K 85.1(2) . 3_656 ?
O2 O11 K 137.7(2) 3_666 3_656 ?
O4 O11 K 52.31(19) 3_656 3_656 ?
K O11 K 146.1(2) 3_666 3_656 ?
C2 O11 OWB 128.6(9) . 3_666 ?
Fe O11 OWB 108.1(8) . 3_666 ?
O7 O11 OWB 67.6(7) . 3_666 ?
O2 O11 OWB 86.2(7) 3_666 3_666 ?
O4 O11 OWB 122.0(7) 3_656 3_666 ?
K O11 OWB 46.4(6) 3_666 3_666 ?
K O11 OWB 99.8(6) 3_656 3_666 ?
C2 O11 K2 77.6(5) . 1_455 ?
Fe O11 K2 167.4(3) . 1_455 ?
O7 O11 K2 123.6(3) . 1_455 ?
O2 O11 K2 137.0(3) 3_666 1_455 ?
O4 O11 K2 131.8(3) 3_656 1_455 ?
K O11 K2 84.38(19) 3_666 1_455 ?
K O11 K2 79.50(19) 3_656 1_455 ?
OWB O11 K2 62.3(8) 3_666 1_455 ?
C2 O11 O8 150.3(7) . 1_545 ?
Fe O11 O8 77.9(2) . 1_545 ?
O7 O11 O8 44.0(2) . 1_545 ?
O2 O11 O8 102.3(2) 3_666 1_545 ?
O4 O11 O8 60.5(2) 3_656 1_545 ?
K O11 O8 103.6(2) 3_666 1_545 ?
K O11 O8 47.34(16) 3_656 1_545 ?
OWB O11 O8 64.3(6) 3_666 1_545 ?
K2 O11 O8 90.2(2) 1_455 1_545 ?
C2 O12 K2 118.8(5) 1_655 . ?
C2 O12 K 116.2(5) 1_655 . ?
K2 O12 K 125.0(3) . . ?
C2 O12 O2 152.1(7) 1_655 . ?
K2 O12 O2 82.4(2) . . ?
K O12 O2 47.57(14) . . ?
OWB OWA O8 127(4) . 4_676 ?
OWB OWA K 51(4) . . ?
O8 OWA K 114.6(7) 4_676 . ?
OWB OWA OWB 121(5) . 2_746 ?
O8 OWA OWB 83(2) 4_676 2_746 ?
K OWA OWB 71.4(15) . 2_746 ?
OWB OWA N2 101(4) . 4_566 ?
O8 OWA N2 132.1(19) 4_676 4_566 ?
K OWA N2 96.8(8) . 4_566 ?
OWB OWA N2 73.5(8) 2_746 4_566 ?
OWB OWA K 126(4) . 2_756 ?
O8 OWA K 58.6(8) 4_676 2_756 ?
K OWA K 169.9(9) . 2_756 ?
OWB OWA K 113(3) 2_746 2_756 ?
N2 OWA K 93.2(9) 4_566 2_756 ?
OWB OWA OWA 109(5) . 2_746 ?
O8 OWA OWA 91.6(18) 4_676 2_746 ?
K OWA OWA 59.9(11) . 2_746 ?
OWB OWA OWA 12.0(8) 2_746 2_746 ?
N2 OWA OWA 73.2(8) 4_566 2_746 ?
K OWA OWA 125(3) 2_756 2_746 ?
OWB OWA OWA 71(4) . 2_756 ?
O8 OWA OWA 76.9(11) 4_676 2_756 ?
K OWA OWA 115(2) . 2_756 ?
OWB OWA OWA 160(3) 2_746 2_756 ?
N2 OWA OWA 122.0(10) 4_566 2_756 ?
K OWA OWA 57.0(11) 2_756 2_756 ?
OWA OWA OWA 164.7(15) 2_746 2_756 ?
OWB OWA O10 96(4) . 2_656 ?
O8 OWA O10 107.5(10) 4_676 2_656 ?
K OWA O10 136.7(14) . 2_656 ?
OWB OWA O10 124.8(18) 2_746 2_656 ?
N2 OWA O10 59.3(4) 4_566 2_656 ?
K OWA O10 48.9(4) 2_756 2_656 ?
OWA OWA O10 129.7(14) 2_746 2_656 ?
OWA OWA O10 64.5(6) 2_756 2_656 ?
OWB OWA OWB 82(5) . 2_756 ?
O8 OWA OWB 70.0(10) 4_676 2_756 ?
K OWA OWB 125(2) . 2_756 ?
OWB OWA OWB 152(3) 2_746 2_756 ?
N2 OWA OWB 120.3(7) 4_566 2_756 ?
K OWA OWB 46.8(12) 2_756 2_756 ?
OWA OWA OWB 162(2) 2_746 2_756 ?
OWA OWA OWB 10.5(7) 2_756 2_756 ?
O10 OWA OWB 61.1(6) 2_656 2_756 ?
OWB OWA O10 82(4) . 1_655 ?
O8 OWA O10 66.4(5) 4_676 1_655 ?
K OWA O10 48.3(4) . 1_655 ?
OWB OWA O10 65.1(6) 2_746 1_655 ?
N2 OWA O10 132.0(7) 4_566 1_655 ?
K OWA O10 124.4(9) 2_756 1_655 ?
OWA OWA O10 61.2(7) 2_746 1_655 ?
OWA OWA O10 104.3(12) 2_756 1_655 ?
O10 OWA O10 168.7(8) 2_656 1_655 ?
OWB OWA O10 107.6(8) 2_756 1_655 ?
OWB OWA OH5 57(4) . 3_666 ?
O8 OWA OH5 146.1(8) 4_676 3_666 ?
K OWA OH5 93.1(12) . 3_666 ?
OWB OWA OH5 126.3(10) 2_746 3_666 ?
N2 OWA OH5 57.2(5) 4_566 3_666 ?
K OWA OH5 91.0(5) 2_756 3_666 ?
OWA OWA OH5 120.2(12) 2_746 3_666 ?
OWA OWA OH5 73.4(12) 2_756 3_666 ?
O10 OWA OH5 44.0(4) 2_656 3_666 ?
OWB OWA OH5 78.1(11) 2_756 3_666 ?
O10 OWA OH5 137.3(15) 1_655 3_666 ?
OWB OWA O8 78(4) . 3_666 ?
O8 OWA O8 136.3(12) 4_676 3_666 ?
K OWA O8 49.3(4) . 3_666 ?
OWB OWA O8 54.0(12) 2_746 3_666 ?
N2 OWA O8 48.7(4) 4_566 3_666 ?
K OWA O8 140.8(11) 2_756 3_666 ?
OWA OWA O8 44.7(9) 2_746 3_666 ?
OWA OWA O8 145(2) 2_756 3_666 ?
O10 OWA O8 104.0(6) 2_656 3_666 ?
OWB OWA O8 153(2) 2_756 3_666 ?
O10 OWA O8 86.4(5) 1_655 3_666 ?
OH5 OWA O8 76.5(7) 3_666 3_666 ?
OWB OWA N2 78(4) . 3_766 ?
O8 OWA N2 49.0(4) 4_676 3_766 ?
K OWA N2 87.3(8) . 3_766 ?
OWB OWA N2 112.4(7) 2_746 3_766 ?
N2 OWA N2 173.8(8) 4_566 3_766 ?
K OWA N2 82.6(5) 2_756 3_766 ?
OWA OWA N2 113.0(10) 2_746 3_766 ?
OWA OWA N2 51.7(7) 2_756 3_766 ?
O10 OWA N2 114.6(6) 2_656 3_766 ?
OWB OWA N2 53.5(6) 2_756 3_766 ?
O10 OWA N2 54.1(4) 1_655 3_766 ?
OH5 OWA N2 118.0(11) 3_666 3_766 ?
O8 OWA N2 136.1(10) 3_666 3_766 ?
OWB OWA P2 136(4) . 4_666 ?
O8 OWA P2 18.5(4) 4_676 4_666 ?
K OWA P2 106.5(6) . 4_666 ?
OWB OWA P2 64.5(18) 2_746 4_666 ?
N2 OWA P2 120.9(15) 4_566 4_666 ?
K OWA P2 69.4(9) 2_756 4_666 ?
OWA OWA P2 73.4(15) 2_746 4_666 ?
OWA OWA P2 95.4(13) 2_756 4_666 ?
O10 OWA P2 116.7(12) 2_656 4_666 ?
OWB OWA P2 88.4(12) 2_756 4_666 ?
O10 OWA P2 60.5(5) 1_655 4_666 ?
OH5 OWA P2 160.3(9) 3_666 4_666 ?
O8 OWA P2 118.1(9) 3_666 4_666 ?
N2 OWA P2 61.9(4) 3_766 4_666 ?
OWB OWA O7 20(4) . 3_666 ?
O8 OWA O7 140.3(12) 4_676 3_666 ?
K OWA O7 64.1(9) . 3_666 ?
OWB OWA O7 127(2) 2_746 3_666 ?
N2 OWA O7 85.1(9) 4_566 3_666 ?
K OWA O7 115.4(8) 2_756 3_666 ?
OWA OWA O7 115.9(19) 2_746 3_666 ?
OWA OWA O7 70.0(17) 2_756 3_666 ?
O10 OWA O7 77.5(7) 2_656 3_666 ?
OWB OWA O7 79.5(18) 2_756 3_666 ?
O10 OWA O7 101.0(11) 1_655 3_666 ?
OH5 OWA O7 37.1(5) 3_666 3_666 ?
O8 OWA O7 75.7(8) 3_666 3_666 ?
N2 OWA O7 92.5(10) 3_766 3_666 ?
P2 OWA O7 153.8(9) 4_666 3_666 ?
OWB OWA OH5 121(4) . 4_666 ?
O8 OWA OH5 36.7(4) 4_676 4_666 ?
K OWA OH5 83.7(5) . 4_666 ?
OWB OWA OH5 52.5(11) 2_746 4_666 ?
N2 OWA OH5 122.9(12) 4_566 4_666 ?
K OWA OH5 92.2(10) 2_756 4_666 ?
OWA OWA OH5 57.9(11) 2_746 4_666 ?
OWA OWA OH5 108.1(11) 2_756 4_666 ?
O10 OWA OH5 139.2(14) 2_656 4_666 ?
OWB OWA OH5 103.9(9) 2_756 4_666 ?
O10 OWA OH5 39.8(3) 1_655 4_666 ?
OH5 OWA OH5 176.8(11) 3_666 4_666 ?
O8 OWA OH5 101.2(6) 3_666 4_666 ?
N2 OWA OH5 62.1(4) 3_766 4_666 ?
P2 OWA OH5 22.9(2) 4_666 4_666 ?
O7 OWA OH5 140.4(10) 3_666 4_666 ?
OWB OWA O8 48(4) . 3_676 ?
O8 OWA O8 115.8(7) 4_676 3_676 ?
K OWA O8 98.1(13) . 3_676 ?
OWB OWA O8 161.2(19) 2_746 3_676 ?
N2 OWA O8 92.8(7) 4_566 3_676 ?
K OWA O8 79.7(5) 2_756 3_676 ?
OWA OWA O8 151(2) 2_746 3_676 ?
OWA OWA O8 38.9(11) 2_756 3_676 ?
O10 OWA O8 52.9(5) 2_656 3_676 ?
OWB OWA O8 46.3(13) 2_756 3_676 ?
O10 OWA O8 120.0(12) 1_655 3_676 ?
OH5 OWA O8 36.7(4) 3_666 3_676 ?
O8 OWA O8 107.2(10) 3_666 3_676 ?
N2 OWA O8 81.9(7) 3_766 3_676 ?
P2 OWA O8 134.3(6) 4_666 3_676 ?
O7 OWA O8 36.2(4) 3_666 3_676 ?
OH5 OWA O8 143.9(7) 4_666 3_676 ?
OWB OWA O7 155(4) . 4_666 ?
O8 OWA O7 35.3(7) 4_676 4_666 ?
K OWA O7 113.4(8) . 4_666 ?
OWB OWA O7 54(2) 2_746 4_666 ?
N2 OWA O7 100.1(12) 4_566 4_666 ?
K OWA O7 66.2(9) 2_756 4_666 ?
OWA OWA O7 64.7(16) 2_746 4_666 ?
OWA OWA O7 108.1(17) 2_756 4_666 ?
O10 OWA O7 106.5(11) 2_656 4_666 ?
OWB OWA O7 99.0(17) 2_756 4_666 ?
O10 OWA O7 74.3(7) 1_655 4_666 ?
OH5 OWA O7 148.0(11) 3_666 4_666 ?
O8 OWA O7 106.6(9) 3_666 4_666 ?
N2 OWA O7 82.5(7) 3_766 4_666 ?
P2 OWA O7 20.8(3) 4_666 4_666 ?
O7 OWA O7 174.5(7) 3_666 4_666 ?
OH5 OWA O7 34.6(4) 4_666 4_666 ?
O8 OWA O7 144.0(7) 3_676 4_666 ?
OWA OWB K 118(4) . . ?
OWA OWB OWA 97(5) . 2_756 ?
K OWB OWA 135(3) . 2_756 ?
OWA OWB O8 43(4) . 4_676 ?
K OWB O8 112.1(12) . 4_676 ?
OWA OWB O8 73.1(14) 2_756 4_676 ?
OWA OWB N2 68(4) . 4_566 ?
K OWB N2 100.3(10) . 4_566 ?
OWA OWB N2 120.6(13) 2_756 4_566 ?
O8 OWB N2 110(2) 4_676 4_566 ?
OWA OWB OH5 114(4) . 3_666 ?
K OWB OH5 108(2) . 3_666 ?
OWA OWB OH5 80.1(11) 2_756 3_666 ?
O8 OWB OH5 139.4(16) 4_676 3_666 ?
N2 OWB OH5 59.2(6) 4_566 3_666 ?
OWA OWB O11 154(5) . 3_666 ?
K OWB O11 65.0(15) . 3_666 ?
OWA OWB O11 71.2(19) 2_756 3_666 ?
O8 OWB O11 110.9(10) 4_676 3_666 ?
N2 OWB O11 139(2) 4_566 3_666 ?
OH5 OWB O11 87.8(17) 3_666 3_666 ?
OWA OWB O7 157(5) . 3_666 ?
K OWB O7 77.6(18) . 3_666 ?
OWA OWB O7 81(2) 2_756 3_666 ?
O8 OWB O7 151.1(15) 4_676 3_666 ?
N2 OWB O7 93.5(11) 4_566 3_666 ?
OH5 OWB O7 43.1(8) 3_666 3_666 ?
O11 OWB O7 46.8(11) 3_666 3_666 ?
OWA OWB OWB 49(4) . 2_746 ?
K OWB OWB 69.7(10) . 2_746 ?
OWA OWB OWB 142(4) 2_756 2_746 ?
O8 OWB OWB 70(2) 4_676 2_746 ?
N2 OWB OWB 66.1(13) 4_566 2_746 ?
OH5 OWB OWB 124.0(14) 3_666 2_746 ?
O11 OWB OWB 131(2) 3_666 2_746 ?
O7 OWB OWB 137(2) 3_666 2_746 ?
OWA OWB OWB 87(5) . 2_756 ?
K OWB OWB 142(3) . 2_756 ?
OWA OWB OWB 9.6(6) 2_756 2_756 ?
O8 OWB OWB 66.1(17) 4_676 2_756 ?
N2 OWB OWB 116(2) 4_566 2_756 ?
OH5 OWB OWB 83.0(11) 3_666 2_756 ?
O11 OWB OWB 80(2) 3_666 2_756 ?
O7 OWB OWB 89(2) 3_666 2_756 ?
OWB OWB OWB 134(4) 2_746 2_756 ?
OWA OWB OWA 60(4) . 2_746 ?
K OWB OWA 59.2(8) . 2_746 ?
OWA OWB OWA 152(3) 2_756 2_746 ?
O8 OWB OWA 79(2) 4_676 2_746 ?
N2 OWB OWA 67.3(11) 4_566 2_746 ?
OH5 OWB OWA 121.6(9) 3_666 2_746 ?
O11 OWB OWA 122.3(18) 3_666 2_746 ?
O7 OWB OWA 126(2) 3_666 2_746 ?
OWB OWB OWA 11.1(6) 2_746 2_746 ?
OWB OWB OWA 144(4) 2_756 2_746 ?
OWA OWB O10 87(4) . 1_655 ?
K OWB O10 50.1(5) . 1_655 ?
OWA OWB O10 108.4(8) 2_756 1_655 ?
O8 OWB O10 63.0(8) 4_676 1_655 ?
N2 OWB O10 126.4(14) 4_566 1_655 ?
OH5 OWB O10 157(2) 3_666 1_655 ?
O11 OWB O10 75.4(10) 3_666 1_655 ?
O7 OWB O10 115.6(19) 3_666 1_655 ?
OWB OWB O10 61.8(9) 2_746 1_655 ?
OWB OWB O10 109.0(14) 2_756 1_655 ?
OWA OWB O10 59.1(5) 2_746 1_655 ?
OWA OWB K 46(4) . 2_756 ?
K OWB K 161(2) . 2_756 ?
OWA OWB K 53.7(14) 2_756 2_756 ?
O8 OWB K 50.2(10) 4_676 2_756 ?
N2 OWB K 82.4(14) 4_566 2_756 ?
OH5 OWB K 89.3(9) 3_666 2_756 ?
O11 OWB K 124.5(11) 3_666 2_756 ?
O7 OWB K 121.3(10) 3_666 2_756 ?
OWB OWB K 95(3) 2_746 2_756 ?
OWB OWB K 44.3(16) 2_756 2_756 ?
OWA OWB K 106(3) 2_746 2_756 ?
O10 OWB K 113.2(16) 1_655 2_756 ?
OWA OWB O8 92(4) . 3_666 ?
K OWB O8 51.8(6) . 3_666 ?
OWA OWB O8 161.9(17) 2_756 3_666 ?
O8 OWB O8 122.7(19) 4_676 3_666 ?
N2 OWB O8 48.6(5) 4_566 3_666 ?
OH5 OWB O8 81.8(8) 3_666 3_666 ?
O11 OWB O8 107.1(17) 3_666 3_666 ?
O7 OWB O8 85.1(12) 3_666 3_666 ?
OWB OWB O8 52.2(9) 2_746 3_666 ?
OWB OWB O8 162.8(16) 2_756 3_666 ?
OWA OWB O8 44.0(6) 2_746 3_666 ?
O10 OWB O8 88.1(7) 1_655 3_666 ?
K OWB O8 127.2(18) 2_756 3_666 ?
OWA OWB O10 74(4) . 2_656 ?
K OWB O10 149.9(14) . 2_656 ?
OWA OWB O10 64.2(8) 2_756 2_656 ?
O8 OWB O10 95.1(16) 4_676 2_656 ?
N2 OWB O10 56.3(7) 4_566 2_656 ?
OH5 OWB O10 45.1(4) 3_666 2_656 ?
O11 OWB O10 118.0(15) 3_666 2_656 ?
O7 OWB O10 84.7(10) 3_666 2_656 ?
OWB OWB O10 110(3) 2_746 2_656 ?
OWB OWB O10 60.1(11) 2_756 2_656 ?
OWA OWB O10 117(2) 2_746 2_656 ?
O10 OWB O10 158(2) 1_655 2_656 ?
K OWB O10 45.1(6) 2_756 2_656 ?
O8 OWB O10 103.0(9) 3_666 2_656 ?
OWA OWB N2 91(4) . 3_766 ?
K OWB N2 94.8(11) . 3_766 ?
OWA OWB N2 53.4(5) 2_756 3_766 ?
O8 OWB N2 48.6(5) 4_676 3_766 ?
N2 OWB N2 158(2) 4_566 3_766 ?
OH5 OWB N2 130.0(15) 3_666 3_766 ?
O11 OWB N2 62.6(8) 3_666 3_766 ?
O7 OWB N2 105.1(17) 3_666 3_766 ?
OWB OWB N2 105.4(18) 2_746 3_766 ?
OWB OWB N2 54.5(9) 2_756 3_766 ?
OWA OWB N2 108.4(12) 2_746 3_766 ?
O10 OWB N2 55.0(5) 1_655 3_766 ?
K OWB N2 78.2(9) 2_756 3_766 ?
O8 OWB N2 142.8(10) 3_666 3_766 ?
O10 OWB N2 113.4(10) 2_656 3_766 ?
OWA OWB P2 135(4) . 3_666 ?
K OWB P2 101(2) . 3_666 ?
OWA OWB P2 67.4(15) 2_756 3_666 ?
O8 OWB P2 139.7(10) 4_676 3_666 ?
N2 OWB P2 84.1(8) 4_566 3_666 ?
OH5 OWB P2 25.4(5) 3_666 3_666 ?
O11 OWB P2 63.2(13) 3_666 3_666 ?
O7 OWB P2 24.1(4) 3_666 3_666 ?
OWB OWB P2 145.7(15) 2_746 3_666 ?
OWB OWB P2 73.7(14) 2_756 3_666 ?
OWA OWB P2 139.4(15) 2_746 3_666 ?
O10 OWB P2 138(2) 1_655 3_666 ?
K OWB P2 97.9(8) 2_756 3_666 ?
O8 OWB P2 95.5(12) 3_666 3_666 ?
O10 OWB P2 61.1(6) 2_656 3_666 ?
N2 OWB P2 108.4(14) 3_766 3_666 ?
OWA OWB O8 125(4) . 3_676 ?
K OWB O8 117(2) . 3_676 ?
OWA OWB O8 43.8(12) 2_756 3_676 ?
O8 OWB O8 116.5(10) 4_676 3_676 ?
N2 OWB O8 98.0(9) 4_566 3_676 ?
OH5 OWB O8 41.0(6) 3_666 3_676 ?
O11 OWB O8 61.8(11) 3_666 3_676 ?
O7 OWB O8 41.4(7) 3_666 3_676 ?
OWB OWB O8 164.0(17) 2_746 3_676 ?
OWB OWB O8 50.4(12) 2_756 3_676 ?
OWA OWB O8 162.2(13) 2_746 3_676 ?
O10 OWB O8 134.0(17) 1_655 3_676 ?
K OWB O8 81.0(7) 2_756 3_676 ?
O8 OWB O8 118.8(14) 3_666 3_676 ?
O10 OWB O8 56.2(5) 2_656 3_676 ?
N2 OWB O8 89.0(10) 3_766 3_676 ?
P2 OWB O8 23.5(4) 3_666 3_676 ?
OWA OWB O2 155(4) . . ?
K OWB O2 38.9(11) . . ?
OWA OWB O2 108(3) 2_756 . ?
O8 OWB O2 140.1(12) 4_676 . ?
N2 OWB O2 103.2(12) 4_566 . ?
OH5 OWB O2 76.9(14) 3_666 . ?
O11 OWB O2 40.6(8) 3_666 . ?
O7 OWB O2 39.1(8) 3_666 . ?
OWB OWB O2 106(2) 2_746 . ?
OWB OWB O2 117(3) 2_756 . ?
OWA OWB O2 94.9(16) 2_746 . ?
O10 OWB O2 80.1(11) 1_655 . ?
K OWB O2 159.0(16) 2_756 . ?
O8 OWB O2 67.0(9) 3_666 . ?
O10 OWB O2 121.7(15) 2_656 . ?
N2 OWB O2 98.5(14) 3_766 . ?
P2 OWB O2 63.1(12) 3_666 . ?
O8 OWB O2 78.2(14) 3_676 . ?
 
_refine_diff_density_max    0.796
_refine_diff_density_min   -0.422
_refine_diff_density_rms    0.106



